PHYSICAL REVIEW B 81, 094108 共2010兲

Anomalies in the response of V, Nb, and Ta to tensile and shear loading: Ab initio density functional theory calculations Naoyuki Nagasako,1,* Michal Jahnátek,2,† Ryoji Asahi,1,‡ and Jürgen Hafner2,§ 1

Toyota Central Research and Development Laboratories Inc., Nagakute, Aichi 480-1192, Japan Faculty of Physics and Center for Computational Materials Science, University of Vienna, Sensengasse 8/12, A-1090 Wien, Austria 共Received 21 December 2009; revised manuscript received 9 February 2010; published 17 March 2010兲

2

Ab initio density functional calculations of the response of V, Nb, and Ta to tensile and shear loading have been performed. We find that the behavior of all three metals of the V group under large strains differs considerably from that reported for the other body-centered cubic 共bcc兲 transition metals 共Mo, W, and Fe兲. Under unaxial 具100典 tensile loading, V and Nb undergo a bifurcation from a tetragonal to an orthorhombic deformation path, associated with a shear instability, before reaching the stress maximum. The bifurcation strongly reduces the ideal tensile strengths to 11.5 GPa for V and 12.5 GPa for Nb. For Ta the bifurcation point coincides with the stress maximum of 13.6 GPa along the tetragonal path so that the metal fails under tensile strain by shear and not by cleavage. The stress-strain curves calculated for the 兵110其具111典 and 兵211其具111典 slip systems are strongly asymmetric; the ideal shear strengths for both slip systems are 6.5 共5.5兲 GPa for V and 7.8 共6.0兲 GPa for Nb. Hence the ideal shear strengths are only half as large as for the bcc metals Mo and W, but much larger than expected on the basis for the low shear moduli of V and Nb. Ta shows a behavior intermediate between these two groups of metals, with a calculated ideal shear strength of 7.1 共6.5兲 GPa, in excellent agreement with the experimental estimate from nanoindentation experiments. The saddle-point structure determining the shear strength for both slip systems is a special body-centered-tetragonal structure. This structure is identical to the saddle-point structure identified on the orthorhombic deformation path under uniaxial tension. Hence also V and Nb will fail under uniaxial tension not by cleavage, but by shear. DOI: 10.1103/PhysRevB.81.094108

PACS number共s兲: 61.72.Nn, 62.25.⫺g, 62.20.F⫺

I. INTRODUCTION

The strength of any solid is limited by the ideal or theoretical strength defined by the stress required to yield or break a perfect crystal. The ideal shear strength determines the stress necessary for the nucleation of dislocations, while for the formation of a cleavage crack the local stress must exceed the ideal tensile strength.1 In real solids the maximum attainable stress is strongly influenced by the formation of mobile dislocations, by grain boundaries, cracks, and other microstructural features, but it can never exceed the ideal value. While no experimental determinations of the ideal strength under tension have been possible to date, the ideal shear strength can be estimated from nanoindentation experiments.2–6 In nanoindentation experiments the indenter is so small that the volume of the probe undergoing shear deformation may be considered as defect free. In a typical nanoindentation test force and displacement are recorded as the indenter tip is pressed into the materials surface. The yield stress is identified by the first point at which the experimental data deviate from the elastic curve. At this point the indenter moves into the substrate without a measurable increase of the load—this is usually interpreted as a homogeneous dislocation nucleation event.5,6 However, a detailed analysis of the load/displacement curves and detailed molecular dynamics simulations suggest that the nominally “elastic” part of the curve might contain some superimposed plastic deformation too subtle to be detected. This would mean that even nanoindentation experiments can seriously underestimate the theoretical strength. For example, Biener et al.4 derived for body-centered cubic Ta a maximal shear stress of 7.5 GPa, considerably below the theoretical shear 1098-0121/2010/81共9兲/094108共13兲

strength of 11 GPa estimated from the shear modulus of 69 GPa. In view of the difficulty to determine the ideal strength in experiments, there is a continuing interest in its theoretical calculations. The earliest attempts assumed a simple analytic form of the stress-strain curve which allows to derive the ideal strength from the elastic moduli.1,7 This allows to define a dimensionless shear and tensile strength, 쐓 = max / E and 쐓 = max / G, where max and max are the maxima of tensile and shear stress and E and G are the experimental values of the Young’s modulus and the shear modulus for the direction of loading. The reduced dimensionless shear and tensile strengths are assumed to be essentially constant for a specific class of materials. A significant step forward was realized since the 1970s using atomistic models based on empirical or semiempirical force fields which provided valuable information on the atomistic mechanisms of the deformation under large strains.8–12 However, because the parameters of the force fields were necessarily fitted to the materials properties at small strains, the predictions cannot be considered as quantitatively reliable. Finally since the 1990s ab initio density functional calculations began to supercede empirical methods for the determination of the response of metals and intermetallic compounds to tensile and shear loading.13–24 These methods are free from adjustable parameters, valid at all strains and permit in principle a quantitative determination of the ideal strengths. However, because of the relatively large computational effort required in such calculations, early studies were performed at fixed strains.13,14 In this case the selected strain was stepwise increased by small increments while the other five independent strains were fixed at zero, i.e., all internal relaxations were suppressed.

094108-1

©2010 The American Physical Society

PHYSICAL REVIEW B 81, 094108 共2010兲

NAGASAKO et al.

More meaningful results for the energy-strain and stressstrain relations are achieved if the crystal is relaxed until only the stress conjugate to the applied strain has a nonzero value. A review of semiempirical and ab initio calculations of ideal tensile and shear strengths has recently been compiled by Pokluda et al.25 Even to date, ab initio calculations of tensile and shear strengths are available only for a few selected metals and for a very few intermetallic compounds. The face-centered cubic 共fcc兲 metals Al 共Refs. 18, 22–24, and 26–29兲 and Cu 共Refs. 18, 22–24, 30, and 31兲 have been studied most extensively. Among the body-centered cubic metals attention was focused on Fe 共Refs. 32 and 33兲 and on the refractory metals Mo and W.16,19,21 The studies of the fcc metals Al and Cu have emphasized that estimates of the ideal strength based on the elastic be¯ 典 and havior are of limited validity: for both 兵111其具112 ¯ 兵111其具110典 shear deformations, the shear constants of Cu are much higher than those of Al, while from the position of the maximum on the stress-strain curve a higher ideal shear strength is predicted for Al.24,28 The investigations of the loading behavior of the fcc metals have also demonstrated that the theoretical strength may be limited by a shear-related instability, by the softening of a phonon mode along a tensile deformation path or by stacking-fault formation along a shear deformation path, even before the maximum in the stress-strain curve has been reached. For example, the ideal tensile strength 共ITS兲 of Cu under 关100兴 loading is limited by the occurrence of a shear instability30,34 at a strain of 10%. The instability induces a bifurcation from a tetragonal to an orthorhombic deformation path and limits the ITS to 9.5 GPa, compared a stress maximum of 23.8 GPa at a strain of 36.0%. For Al Clatterbuck et al.26 have reported phonon instabilities under uniaxial 关100兴 tension at strains of 17% and 18% limiting the ITS to 9.2 GPa compared to a peak value of 12.9 GPa, under 关110兴 tension a soft phonon mode appears at a strain of 11%. In all cases the soft phonon modes show displacement patterns corresponding to periodic shear defor¯ 典 and 兵111其具1 ¯ 10典 shear mations. For Al under both 兵111其具112 deformations the ideal shear strength 共ISS兲 is limited by 共i兲 stacking fault instabilities and 共ii兲 soft phonon modes.24,26 ¯ 典 shear the unstable stacking fault configuUnder 兵111其具112 ration is reached at a strain of 14.5%, at the same strain a phonon instability has been reported. The displacement of ¯ 典 shear failthe soft phonon mode corresponds to 兵111其具112 ure with a periodicity of two or three 兵111其 planes, it is also closely related to the failure mode induced by the soft phonon mode predicted for 关110兴 tension 共for a detailed discussion we refer to Jahnátek et al.兲24 For fcc Cu, no shear instabilities occur under uniaxial 关110兴 or 关100兴 tensile loading. Also, in contrast to Al the unstable stacking fault configura¯ 典 and 兵111其具1 ¯ 10典 shear deformations tions under 兵111其具112 are reached only at strains beyond the maximum on the stress-strain curve.23,24,34 In comparison to this very complex scenario, the investigations of the bcc metals presented so far describe a much simpler picture. Investigations of tensile loading have concentrated on the 具100典 directions because symmetry

considerations,12 early ab initio calculations16 and empirical tests have all identified the 具100典 directions as the weak directions in tension and the 兵100其 planes as cleavage planes. The general theory of the response of cubic metals to uniaxial loading along 具100典 has been developed in a series of classical papers by Milstein et al.10,11 Starting from an unstressed bcc structure all metals first adopt a primary deformation path with tetragonal guiding symmetry. Any deviation from tetragonality implies the presence of a transverse load. However, as already shown by Hill and Milstein8 at a “special invariant state” where the elastic constants satisfy the condition c22 = c23, a bifurcation to a secondary orthorhombic path may occur under dead load 共note that the invariance condition implies a tetragonal shear instability兲. For the refractory bcc metals Mo and W 共Refs. 19 and 21兲 and for bcc Fe 共Ref. 32兲 it has been shown that the tetragonal symmetry is broken only after the point of maximum tensile stress has been passed. Only for bcc Nb the bifurcation occurs already at a lower strain and leads to an ITS which is significantly lower 共13.1 GPa兲 than that on the tetragonal path 共18.8 GPa兲. Shear deformations along 具111典 may occur in bcc crystals by slip on the 共110兲, 共112兲, and 共123兲 planes. All three shear systems have been studied by Roundy et al.19 for W, while for Mo, Nb, and Fe only the two first have been investigated. The stress-strain curves are very similar for 关111兴 slip along all investigated glide planes, leading to similar values of the ISS. A remarkable result is that for all bcc metals with the exception of Nb the reduced dimensionless tensile and shear strengths are very close to the ideal values, 쐓 = max / E = 0.08 and 쐓 = max / G = 0.11, calculated under the assumption of a sinusoidal stress-strain curve with a period that is twice the strain required to reach the saddle-point structure determining the ideal strength 共i.e., the fcc phase in tension and a body-centered tetragonal phase under shear兲. The stress-strain curve of Nb under shear shows a strong deviation with a low initial slope caused by a low shear modulus, the reduced ideal shear strength is 쐓 = 0.18, i.e., 50% higher than for the other bcc metals. Together these results show that among all investigated bcc metals Nb is the only one that is predicted to fail by 兵211其具111典 shear rather than by 关100兴 tensile failure. In very recent work35 the effect of a superposed transverse stress has been considered. As observed for other metals, hydrostatic tension raises, while hydrostatic compression lowers the ITS of Nb. The exceptional behavior of Nb under tensile and shear loading has been attributed to a very low G具111典 / E具100典 ratio were the relaxed modulus for 关100兴 tension is given by E具100典 =

共c11 − c12兲共c11 + 2c12兲 , c11 + c12

共1兲

3c44共c11 − c12兲 , 4c44 + c11 − c12

共2兲

and G具111典 =

is the relaxed modulus for shear along 具111典 共note that because of the threefold rotational symmetry around the 具111典 axes, any shear in this direction has the same modulus兲. Using the experimental values of the elastic constants36–40 this

094108-2

PHYSICAL REVIEW B 81, 094108 共2010兲

ANOMALIES IN THE RESPONSE OF V, Nb, AND Ta TO…

ratio is G / E = 0.34, 0.28, and 0.42 for V, Nb, and Ta, and G / E = 0.35 and 0.39 for Mo and W. This would suggest that the anomalous behavior under tensile and shear loading should be restricted to Nb, while V and Ta should be expected to behave similarly as Mo and W. However, it is well known that Nb and V share some interesting anomalies in their elastic, dynamic, and superconducting properties: 共i兲 low values of the trigonal and tetragonal shear constants 共c44 = 43, 29, and 83 GPa for V, Nb, and Ta; c⬘ = 共c11 − c12兲 / 2 = 55.5, 57 and 53 GPa for V, Nb, and Ta兲. 共ii兲 Theoretical calculations41,42 predict a pronounced softening of the trigonal shear modulus of V and Nb under compression, driving a mechanical instability of bcc V while for Nb the shear modulus softens for pressures around 50 GPa, but remains positive. The occurrence of a structural phase transition of V from bcc to a rhombohedral phase at about 63–69 GPa has recently been confirmed by synchrotron x-ray diffraction.44 In contrast the absence of pressure-induced phase transitions in Nb up to 145 GPa has recently been confirmed.45 共iii兲 The elastic anomalies of V and Nb are reflected in anomalies of their phonon dispersion relations.46–48 共iv兲 Phonon softening is thought to be responsible for the high superconducting transition temperature Tc in Nb and for the strong increase of Tc under compression in V. The elastic and phonon anomalies have been discussed extensively in relation to the electronic properties and shown to be related to the nesting properties of the Fermi surface.42,49 In particular, the downward dispersion of the transverse phonon branch along 关100兴 and therefore also the unusual softness of c44 has been shown to arise from the nesting properties of the Fermi surface around the N point leading to a van Hove singularity in the electronic density of states close to the Fermi energy. Here we present an extended study of the response of all three V-group metals to tensile and shear loading based on ab initio density functional calculations. Our calculations allow for a bifurcation from a tetragonal to an orthorhombic deformation path under uniaxial tensile strain. Shear deformations have been studied for the 兵110其具111典 and 兵211其具111典 shear systems.

The crystal structure was fully relaxed at each deformation step until all lateral stresses vanished. This has been done by the efficient external optimizer GADGET developed by Bučko et al.55 GADGET performs a relaxation in terms of generalized coordinates which allow a better control of lateral stresses. The forces acting on the atoms were computed via the Hellmann-Feynman theorem,56 the stress tensor acting on the unit cell was computed via the generalized virial theorem.57 The use of a high cut-off energy allows to achieve a high accuracy of the components of the stress tensor. The Brillouin zone 共BZ兲 was sampled using various types of meshes according to the size and symmetry of the computational cells. Because the elastic properties and the stresses at small strains of V and Nb are strongly influenced by the occurrence of van Hove anomalies close to the Fermi level, very fine k-point meshes 共up to 23⫻ 23⫻ 23 for calculations based on a simple face-centered or body-centered tetragonal cell and up to 22⫻ 14⫻ 8 for the larger supercells used for simulating shear deformations兲 are required to calculate the elastic shear constants and the stress-strain relations. All integration meshes were constructed according to the Monkhorst-Pack scheme.58 The integration over the BZ used the Methfessel-Paxton method59 with the smearing parameter of 0.2 eV for calculation of the total energies and stresses, and the tetrahedron method with Blöchl corrections60 for the calculation of the density of states. The total energy was calculated with high precision, converged to 10−8 eV/ atom. The structural relaxation was stopped when all forces acting on the atoms where converged to within 10−3 eV/ Å and all components of the stress tensor except that conjugate to the imposed strain where converged to within 0.05 GPa. For the calculation of the elastic constants we used the linear-interpolation method of the stress tensors. The cubic cells were submitted to the ⫾1 and ⫾4 strains; the tetragonal cells were submitted in addition to ⫾3 and ⫾6 strains; for the orthorhombic cells two more strains, ⫾2 and 5; were added. For each set of strains ⫾i two different magnitudes of 0.2% and 0.5% were used. For the calculation of the elastic constants the total energy was calculated with even higher accuracy, converged to 10−9 eV/ atom.

II. COMPUTATIONAL METHODS

III. ELASTIC PROPERTIES

Our ab initio total-energy and force calculations are based on density functional theory 共DFT兲 as implemented in the Vienna ab initio simulation package 共VASP兲.50,51 A gradientcorrected functional has been used to describe electronic exchange and correlations.52 Electron-ion interactions are treated within the projector-augmented wave 共PAW兲 method.53,54 For all elements we used the standard PAW pseudopotentials 共PP兲 distributed with VASP with reference configurations np6nd4共n + 1兲s1 for the valence states with n = 3 , 4, and 5 for V, Nb, and Ta. The plane-wave basis set contained components with kinetic energies up to 350 eV. The response of the crystal to tensile or shear deformations was calculated by increasing the strain along the chosen directions in small steps. Increasing/decreasing the strain by very small increments leads to a reversible deformation process at zero absolute temperature with negligible hysteresis.

The elastic constants of the V-group metals, together with the Young’s modulus E具100典 for tension along 具100典 and the relaxed shear modulus G具111典 for shear along the 具111典 direction are compiled in Table I. It is well known that although very good agreement for the bulk modulus 关B = 共c11 + 2c12兲 / 3兴 and the orthorhombic shear constant c⬘ = 共c11 − c12兲 / 2 is achieved, all DFT calculations seriously underestimate the trigonal shear constant c44, irrespective of the exchange-correlation functional 共local or semilocal gradientcorrected functional兲 and of the method used for solving the Kohn-Sham equations 共plane-wave based pseudopotential or PAW calculations, muffin-tin orbital methods兲.41–43 The low value of the trigonal shear constant is related to an anomalous dispersion of transverse acoustic phonons propagating along the 具100典 direction. In the long-wavelength limit, shear constant, and frequencies of transverse acoustic phonons are

094108-3

PHYSICAL REVIEW B 81, 094108 共2010兲

NAGASAKO et al.

TABLE I. Elastic constants, shear anisotropy A = 2共c⬘ − c44兲 / c44, relaxed tensile modulus E具100典, relaxed shear modulus G具111典, and ratio G/E for the body-centered cubic metals of the V group 共in GPa兲. Metal V

Nb

Ta

Mo

W

Reference

c11

c12

c44

c⬘ = 共c11 − c12兲 / 2

A

E具100典

G具111典

G/E

This work Theory, Ref. 42 Theory, Ref. 43 Exp., Ref. 37 This work Theory, Ref. 42 Theory, Ref. 43 Exp., Ref. 37 This work Theory, Ref. 42 Theory, Ref. 43 Exp., Ref. 37 This work Theory, Ref. 43 Exp., Ref. 37 This work Theory, Ref. 43 Exp., Ref. 37

262 260 205 231 247 247 267 246 257 265 291 266 470 406 465 500 553 523

144 135 130 120 138 138 147 133 163 159 162 161 161 150 162 205 207 204

17 17 5 43 17 10 27 29 71 74 84 83 105 107 109 130 178 161

59 63 37.5 55.5 54.5 54.5 60 57 47 53 64.5 53 154 128 152 148 173 159

4.9 5.4 13.0 0.56 4.4 8.9 2.4 1.9 −0.68 −0.57 −0.46 −0.72 0.93 0.40 0.78 0.27 −0.06 0.03

160 168 104 149 148 148 163 154 132 146 175 145 386 325 381 382 440 407

32 33 12 50 31 22 43 43 53 59 70 60 133 120 134 142 175 159

0.20 0.20 0.11 0.33 0.21 0.15 0.26 0.28 0.40 0.40 0.40 0.41 0.34 0.37 0.35 0.37 0.40 0.39

related through c44 = 2共q兲 / q2 where is the density. Softening of acoustic phonons and the low value of the shear constant are related to the nesting properties of the Fermi surface which produce a van Hove singularity in the electronic density of states 共DOS兲 close to the Fermi level, as discussed in detail by Landa et al.41 As shown in Fig. 1, the distance between the van-Hove peak in the DOS and the Fermi energy increases from V to Nb and Ta, in correspondence to an increasing value of the shear constant. Due to the presence of the van-Hove singularity, an exact determination of c44 requires a very fine mesh for Brillouin zone integrations. With a 23⫻ 23⫻ 23 grid, full convergence is achieved, but the shear constant is still too low by a factor of about two. It is well known that crystalline imperfections tend to smear out the Fermi surface and hence the singularity in the DOS and that this results in a damping of the related anoma-

Total DOS (states/eV/cell)

3.5

bcc-V bcc-Nb bcc-Ta

3.0

lies in the phonon dispersion relations and to a stiffening of the elastic shear modes. In theoretical calculations this effect may be modeled by applying a Gaussian smearing to the eigenstates and we find that a broadening of the energy levels leads to a larger value of the c44 shear constant. While this might account for part of the discrepancy between theory and experiment, more accurate experiments at low temperatures and high-quality specimens would also be desirable. For the moment we note that the very low values resulting from all theoretical calculations should be treated with caution, although the trends among the V-group metals are at least semiquantitatively correct. We also note that for the relaxed tensile and shear moduli relevant to the present study, agreement between theory and experiment is better than for c44 alone. To assess the validity of our method for calculating the elastic constants of bcc transition metals we include in Table I our results for Mo and W, together with the experimental values. For both metals we note very good agreement between theory and experiment.

2.5

IV. RESPONSE TO UNIAXIAL [100] TENSILE LOADING

2.0 1.5 1.0 0.5 0.0 -8

-6

-4

-2

0

2

Energy (eV)

FIG. 1. 共Color online兲 Electronic density of states of bcc V, Nb, and Ta. Note the van-Hove singularities close to the Fermi level.

The general theory of the response of cubic metals to uniaxial 具100典 loading has been formulated by Milstein et al.8,9,11 On the primary tetragonal deformation path 共the Bain path兲 the structure can be considered as either body-centered tetragonal 共bct兲 or face-centered tetragonal 共fct兲. By symmetry only three stress-free states are possible: bcc, fcc, and a special bct 共or equivalently fct兲 structure, but the order of appearance of these states along the deformation path depends on the details of interatomic binding. Owing to crystal symmetry, the fcc state can be reached from the bcc state

094108-4

PHYSICAL REVIEW B 81, 094108 共2010兲

ANOMALIES IN THE RESPONSE OF V, Nb, AND Ta TO… a2 = c

fcc

0.40

fct

a1 = b1 = a

Tetragonal path a3 = 2 a ′ 2

b3 = a′

b2 = a′

a3 = c

(b) Saddle-point structure ~ y y a3 = a0 ~ z

a1 = b1 = a0

(c) Structure at local energy-minimum

b2 = 2a0

(a) Unstrained structure Orthorhombic path

bct

c

0.20 0.15 0.10 0.05 0.00

b3 = 2a0

z

b2 = 2c

b3 = 2c

bcc

fct

a0

a0 b1 = 2c

c b3 = 2c b2 = a (d) Saddle-point structure

bcc-V

-0.05

fct

0.0

(a)

0.1

0.2 0.3 Strain

b1 = 2a0

0.4

b3 = a0

(e) Structure at energy-minimum

only by applying uniaxial tension, hence there are three possible orderings of the stress-free states: 共1兲 bcc, bct, fcc 共as found for the alkali metals兲,11 共2兲 bct, bcc, fcc, and 共3兲 bcc, fcc, bct. The centrally located stress-free state is necessarily unstable because of a decreasing stress at increasing strain, it represents a saddle point on the energy-strain curve. Scenario 共3兲 is realized along the tetragonal deformation path of the bcc transition metals such as W.18–20 If the primary tetragonal path 共PTP兲 contains the “special invariant state” where c22 = c23, a bifurcation to a secondary orthorhombic path 共SOP兲 can occur under strict uniaxial load. Immediately after bifurcation the system passes through a stress-free bct state while at larger strain the original bcc structure is recovered. Figure 2共a兲 shows a sketch of the bcc lattice embedded into a more general fct lattice. Tetragonal deformations can be described by the variation of the lattice parameters a1 and a2 = a3 of a bct lattice with a1 increasing linearly as a function of strain. The deformations along an orthorhombic deformation path can be described in terms of a fct lattice with b1 = a1 = a0 and b2 = b3 = 冑2a0 in the undeformed state. Along the PTP relaxation minimizes the total energy with respect to a2 = a3 only, while along the SOP the total energy is minimized independently with respect to both b2 and b3. The energy-strain and stress-strain curves, as well as the variation in the lattice parameters ai and bi as a function of strain are shown for V, Nb, and Ta in Figs. 3–5. As a measure of strain we use the engineering strain. The scenario is qualitatively the same for all three metals, albeit with some important quantitative differences. Along the PTP the maximum on the energy-strain curve is the fcc structure as shown in Fig. 2共b兲. Under a volume-conserving deformation the strain at which the bct cell assumes the fcc structure is given by the Bain strain of ⑀B = 冑3 2 − 1 = 0.26. For all three metals the fcc structure is realized at a slightly larger strain varying from ⑀ = 0.274 for V to ⑀ = 0.273 for Nb and ⑀ = 0.271 for Ta,

Orthorhombic path Tetragonal path

bcc-V 0.0

(b)

0.1

0.2 0.3 Strain

0.4

0.5

bcc-V

5.0

FIG. 2. 共Color online兲 Sketch of the PTP and SOP deformation paths of a body-centered cubic lattice shown in red 共black兲 under uniaxial 关100兴 tensile loading. The structures along the PTP are described within the body-centered tetragonal reference frame 共lattice constants ai , i = 1 – 3兲, those along the SOP are described as face-centered tetragonal 关shown in blue 共gray兲—lattice constants bi , i = 1 – 3兴.

30 25 20 15 10 5 0 -5 -10 -15 -20 -25 -30

5.5

a0 b2 = 2a0

0.5

4.5 4.0 3.5 3.0 2.5

b1 (OP) b2 (OP) b3 (OP) a1 (TP) a2, a3 (TP)

2.0 1.5 1.0 0.0

(c)

0.1

0.2

0.3

0.4

0.5

Strain

FIG. 3. Variation in 共a兲 the total energy, 共b兲 the stress, and 共c兲 the lattice constants of bcc V under 关100兴 tension as a function of the applied strain. Open symbols refer to the primary tetragonal deformation path, closed symbols to the secondary orthorhombic deformation path. The bifurcation from the PTP to the SOP occurs at a strain of 0.06.

corresponding to a slight volume expansion. Upon further increased tensile strain the total energy reaches a minimum for a special bct structure at ⑀ = 0.494 for V, ⑀ = 0.479 for Nb and at ⑀ = 0.438 for Ta. The ITS and the critical strains for all three metals calculated along the PTP are compiled in Table 0.40

Orthorhombic path Tetragonal path

0.35 0.30 0.25

σ11 (GPa)

bcc

fct

0.25

Lattice parameters (A)

x ~ x

0.30

0.20 0.15 0.10 0.05 0.00

bcc-Nb

-0.05

(a)

0.0

0.1

0.2

0.3

0.4

0.5

Strain

30 25 20 15 10 5 0 -5 -10 -15 -20 -25 -30

(b)

Orthorhombic path Tetragonal path

bcc-Nb 0.0

0.1

0.2 0.3 Strain

0.4

0.5

5.5 bcc-Nb

5.0 Lattice parameters (A)

a 2 = a0

Orthorhombic path Tetragonal path

0.35

σ11 (GPa)

a1 = b1 = a′

bct

∆E = E(ε) - E(0) (eV/atom)

bct

∆E = E(ε) - E(0) (eV/atom)

a2 = 2 a′ 2

4.5 4.0 3.5 3.0 2.5

b1 (OP) b2 (OP) b3 (OP) a1 (TP) a2, a3 (TP)

2.0 1.5 1.0

(c)

0.0

0.1

0.2 0.3 Strain

0.4

0.5

FIG. 4. Variation in 共a兲 the total energy, 共b兲 the stress, and 共c兲 the lattice constants of bcc Nb under 关100兴 tension as a function of the applied strain. Open symbols refer to the primary tetragonal deformation path, closed symbols to the secondary orthorhombic deformation path. The bifurcation from the PTP to the SOP occurs at a strain of 0.05.

094108-5

PHYSICAL REVIEW B 81, 094108 共2010兲

NAGASAKO et al. 0.40

0.25 σ11 (GPa)

∆E = E(ε) - E(0) (eV/atom)

0.30

0.20 0.15 0.10 0.05 0.00

bcc-Ta

-0.05

(a)

30 25 20 15 10 5 0 -5 -10 -15 -20 -25 -30

Orthorhombic path Tetragonal path

0.35

0.0

0.1

0.2 0.3 Strain

0.4

0.5

(b)

Orthorhombic path Tetragonal path

bcc-Ta 0.0

0.1

0.2

0.3

0.4

0.5

Strain

5.5 bcc-Ta

Lattice parameters (A)

5.0 4.5 4.0 3.5 3.0 2.5

b1 (OP) b2 (OP) b3 (OP) a1 (TP) a2, a3 (TP)

2.0 1.5 1.0

(c)

0.0

0.1

0.2

0.3

0.4

0.5

Strain

FIG. 5. Variation in 共a兲 the total energy, 共b兲 the stress, and 共c兲 the lattice constants of bcc Ta under 关100兴 tension as a function of the applied strain. Open symbols refer to the primary tetragonal deformation path, closed symbols to the secondary orthorhombic deformation path. The bifurcation from the PTP to the SOP 共equivalent to a shear instability of the bct lattice兲 occurs at a strain of ⑀ = 0.16, i.e., it is almost coincident with the stress maximum along the PTP.

II. For Nb we note a very good agreement with the results of Luo et al.21 The dimensionless ITSs 쐓 = max / E具100典 ⬃ 0.10– 0.11 reached along the PTP are somewhat larger than those calculated of bcc Mo and W, reflecting a modest asymmetry of the stress-strain curve. If the constraint of a tetragonal guiding symmetry is relaxed, a bifurcation to the SOP occurs at low values of the critical strain, ⑀c = 0.06 and 0.05 for V and Nb, but only at ⑀c = 0.16 for Ta. For Ta this critical strain is almost identical to the critical strain at which the stress maximum is reached along the PTP, while for V and Nb the ITS is limited by the bifurcation to the SOP. Figure 6 shows the variation in the elastic constants of all three metals under uniaxial strain along the 关100兴 direction, referred to a face-centered tetragonal lattice. The important

results are the following: 共i兲 within a fct reference frame the condition c22 = c23 is fulfilled at strains of 0.06, 0.05, and 0.18 for V, Nb, and Ta, respectively. Within a bct reference frame, the condition for a bifurcation is c44 = 0. 共ii兲 At these strains the symmetry will change from tetragonal to orthorhombic under purely uniaxial loading. The behavior of V and Nb at the bifurcation point differs substantially from that of Ta. For V and Nb the energy-strain curves of the PTP and SOP are tangent at the bifurcation point, the difference between the lattice constants b2 and b3 changes continuously, the stress continues to increase after the bifurcation. Hence for V and Nb the branching from the PTP to the SOP is a continuous second order structural transformation from the bct to a face-centered orthorhombic structure induced by purely uniaxial loading which occurs before the ideal tensile strength is reached. For Ta the condition c22 = c23 共within the fct reference frame兲 or c44 = 0 共within a bct description of the deformed structure兲 leads to a shear instability at the stress maximum under uniaxial tension. This means that even under strict uniaxial load, Ta fails not by cleavage but by shear. The unstable saddle-point configuration reached along the SOP is a “special” bct structure which is energetically degenerate with the metastable fct structure reached at large strains on the PTP. In fact, both structures are related through a rigid rotation about the b3 axis, the axial ratio of the fct structure is just 1 / 冑2 times the axial ratio of the bct structure 共a1 / a2 = 1.81兲. At a strain of about 0.41 the energy along the SOP falls to an energy minimum. The configuration corresponding to this minimum is a bcc structure rotated about the b2 axis relative to the original bcc structure. The restoring strain of ⑀ = 0.41 is very close to the value of ⑀ = 冑2 − 1 = 0.414 calculated for a strictly volume-conserving deformation. The bct saddle-point configuration reached on the SOP under uniaxial 具100典 loading is identical to that reached under shear along a 具111典 axis, as will be discussed in more detail below. Hence also along the SOP the bcc metals are predicted to fail not by cleavage, but by shearing. Hence we find that along the PTP the sequence of the stress-free structures is bcc, fcc, bct 关corresponding to scenario 共3兲 discussed by Milstein et al.8,9,11兴 for V, Nb, and Ta, as for the other bcc transition metals 共Mo, W, Fe兲 investigated so far. For Ta the criterion c22 = c23 for a bifurcation to an orthorhombic path is satisfied only for a large strain co-

TABLE II. Ideal tensile strengths max, critical strain ⑀c, Young’s modulus E关100兴 of V, Nb and Ta under uniaxial 关100兴 loading, as determined by the stress maximum along the tetragonal and orthorhombic deformation paths. Orthorhombic

V Nb Ta Mo W

This work This work Ref. 21 This work Ref. 21 Ref. 19

Tetragonal

E具100典

max

⑀c

max / E具100典

max

⑀c

max / E具100典

160 148 165 146 370 407

11.5 12.5 13.1 13.6

0.10 0.11 0.12 0.16

0.07 0.09 0.08 0.09

17.8 17.2 18.8 13.4 28.8 29.5

0.17 0.17 0.18 0.16 0.13 0.13

0.11 0.12 0.11 0.10 0.08 0.07

094108-6

PHYSICAL REVIEW B 81, 094108 共2010兲

ANOMALIES IN THE RESPONSE OF V, Nb, AND Ta TO… 300

300

bcc-V (related to a fct lattice)

200

c11 c12 c22 c23 c44 c55

150 100 50 0 -50 0.00

0.05

0.10

0.15

0.20

0.25

50

0.05

0.10

0.15

0.20

0.25

0.30

Strain 300

bcc-Nb (related to a fct lattice)

bcc-Ta (related to a fct lattice)

250

200

Elastic constant (GPa)

Elastic constant (GPa)

100

(b)

250 c11 c12 c22 c23 c44 c55

150 100 50 0

(c)

c11 c12 c22 c23 c44 c55

150

-50 0.00

0.30

Strain

-50 0.00

200

0

(a) 300

bcc-V (related to a bct lattice)

250 Elastic constant (GPa)

Elastic constant (GPa)

250

200

c11 c12 c22 c23 c44 c55

150 100 50 0

0.05

0.10

0.15 Strain

0.20

0.25

-50 0.00

0.30

(d)

0.05

0.10

0.15 Strain

0.20

0.25

0.30

FIG. 6. 共Color online兲 Variation in the elastic constants c11, c12, c22, c23, c44, and c55 共related to a face-centered tetragonal lattice兲 of 共a兲 V, 共c兲 Nb, and 共d兲 Ta along the primary tetragonal deformation path as a function of uniaxial 关100兴 strain. For V we show also the elastic constants related to a bct reference frame 共b兲, in this case the elastic constants reduce to c11, c12, and c44 in the bcc limit. Note that the condition for the bifurcation to an orthorhombic lattice is c22 = c23 in the fct reference frame 共contraction/expansion along the fct axes—cf. Fig. 2兲, but c44 = 0 in the bct reference frame 共contraction/expansion along the face-diagonals of the bct basis plane兲.

incident with the critical strain for tensile failure along the PTP. Hence the situation is similar to that described before for Mo 共Ref. 21兲 and Fe.32 If the saddle-point structure on the SOP is described within the bct reference frame used for tetragonal deformation under 关100兴 tension, the orthorhombic instability corresponds to a shear instability with c44 = 0. For V and Nb the bifurcation to the SOP occurs already at much smaller strains, the failure mode is determined by the fct saddle-point structure along the SOP. The ITS is reduced from 17.8 GPa to 11.5 GPa for V, and from 17.2 to 12.5 GPa for Nb. The value for Nb is in good agreement with the earlier calculations of Luo it et al.21 For Ta the stress maximum is 13.4 GPa along the tetragonal and 13.6 GPa along the orthorhombic deformation path, i.e the values agree within the computational accuracy. For all three metals the stress-strain curves along the PTP are too asymmetric to be fitted by a sinusoidal curve, leading to a dimensionless ITS of 쐓 ⬃ 0.10– 0.12 which is larger than that calculated for the other bcc transition metals. The stress-strain curve for the SOP is more symmetric, the dimensionless ITS assumes values of 0.07 to 0.09 comparable with those derived for Mo, W, and Fe. V. RESPONSE TO SHEAR DEFORMATIONS ALONG THE Š111‹ DIRECTION

Figure 7 shows the computational cells used for simulating shear deformations along a 具111典 direction on the 兵211其

and 兵110其 planes. The undeformed cells are orthorhombic, with lattice parameters aSC, bSC, and cSC as defined in the figure. The shear deformation was applied uniformly to the supercell 共affine shear loading兲. This means that in principle, the calculations could also have been performed with a primitive cell instead. The supercells have been used for computational convenience. With current optimizer relaxation of all transverse stress components to zero values is easier in the supercell geometry. Because of the threefold rotational symmetry around the 具111典 axis the relaxed shear modulus G具111典 is the same for all common bcc slip systems, 兵110其具111典, 兵211其具111典, and 兵321其具111典 共here we discuss only the former two兲. Earlier work of Morris et al.19–21,61 on the response of W and Mo to shear loading has demonstrated that the relaxed energy/ strain, stress/strain curves, and the ideal shear strengths are very similar for all three slip systems. The changes in symmetry during shear deformation have been discussed in detail by Roundy et al.19 and Krenn et al.,20 using slightly different geometrical arguments. The 兵110其具111典 shear system is symmetric, while the 兵211其具111典 and 兵321其具111典 are not, i.e., slip in the “easy” direction has a lower shear strength than in the “hard” direction. Here we shall restrict our attention to slip in the easy 共weak兲 direction. Upon shearing the bcc lattice parallel to the 共211兲 plane a mirrored bcc lattice is created at a strain of ␥ = 冑2 / 2 ⬃ 0.71 共the “twining” strain兲 if relaxation is excluded. If only a single maximum in the total energy exists for strains from 0 to 0.71, symmetry dictates that it must be

094108-7

PHYSICAL REVIEW B 81, 094108 共2010兲

NAGASAKO et al.

z : [ 1 1 2]

aSC

aSC

bSC

cSC

bSC

cSC β SC α SC γ SC

x : [111]

b

β

c

a

y : [ 1 10]

β SC

Unstrained structure

α SC

c

β

γ SC

a

b

Saddle-point structure

(a) Supercells used for {211} shear

aSC

cSC

z : [1 1 0] b

β SC

α

α SC

cSC

a

β γ

γ SC

x : [111]

aSC

c

bSC

y : [ 1 1 2]

Unstrained structure

b

α SC β SC

c

α β γ

γ SC

a

bSC

Saddle-point structure

(b) Supercells used for {110} shear FIG. 7. 共Color online兲 Supercells used to simulate shear deformations along the 具111典 direction. Part 共a兲 shows the cell used for 兵211其具111典 shear, the left part represents the undeformed cell with bcc symmetry, the right part the bct structure at the saddle-point configuration. The primitive cells inscribed in the supercells are shown in red 共black兲. Part 共b兲 shows the starting 共bcc兲 and saddlepoint 共bct兲 structures for 兵110其具111典 shear. At intermediate strains the symmetry is reduced to monoclinic and triclinic under 兵211其具111典 and 兵110其具111典 shears, respectively. The monoclinic cells inscribed in the supercells which become the bct cells at the saddle-point structure are indicated by the blue 共gray兲 circles.

located at ␥ ⬃ 0.35, and the inflection point must fall around 0.17. Along this deformation path the symmetry changes from cubic to monoclinic and further to orthorhombic at the saddle point 共see Fig. 7兲. For W it has been found that relaxation has only a very small influence on the stress under 共211兲关111兴 strain along the easy direction. This has been attributed to the elastic isotropy of W. Unrelaxed 共110兲关111兴 shear reduces the symmetry from cubic to triclinic, the first energy maximum is found when the deformation path passes through a configuration with monoclinic symmetry. For both Mo and W a significantly stronger relaxation has been reported for 共110兲关111兴—relaxation is necessary to recover the bcc structure at a strain of ␥ ⬃ 0.6. For Mo, Luo et al.21 have reported that due to relaxation, the saddle-point structure under 共110兲关111兴 shear is very similar to the bct saddle point found for the 共211兲关111兴 slip systems. Still, for both Mo and W the stress-strain curves are almost identical for all three slip systems, they have a symmetric sinusoidal shape leading

to a reduced shear strength of max / G具111典 ⬃ 0.11. Luo et al. have also calculated the shear strength of bcc Nb. In this case the stress-strain curves for the 共110兲关111兴 and 共211兲关111兴 shear systems are more distinctly different than for Mo and more asymmetric, leading to a higher value of the reduced shear strength of ⬃0.15– 0.18, although the actual shear strength is much lower. The results for the three V-group metals compiled in Figs. 8–10 show that the response of V and Nb on one side and Ta on the other side are significantly different, although the values of the ideal shear strengths are not. For all three metals the ideal shear strength calculated for both slip systems reaches only half the value found for Mo and W in the neighboring column of the Periodic Table. For V and Nb the stress-strain curves are strongly asymmetric—as we shall show below, this is related to a low value of the shear modulus G具111典, a strong anisotropy of the elastic shear constants 共which is, admittedly, strongly overestimated by the ab initio calculations兲 and strong relaxations under shear loading. For Ta the stress-strain curves are only weakly asymmetric, the reduced shear strength comes close to that calculated for Mo and W. For V, slightly different saddle-point configurations located at strains of 0.28 and 0.32 are found under 兵110其具111典 and 兵211其具111典 shear deformations. These differences are related to different degrees of relaxation changing in both cases significantly as a function of strain. Up to a strain of about 0.08 both shears lead to an increase of the lattice constant bSC, a decrease of cSC, while aSC remains almost constant 关see Figs. 8共c兲 and 8共d兲兴. In this regime only the shearing angle SC increases linearly with strain, while the other angles remain almost unchanged even under 兵110其具111典 shear where the symmetry is reduced to triclinic. Up to this point the deformation occurs at almost constant volume. At a strain of ⑀ = 0.08 the lattice constant cSC reaches a minimum. At larger strains the lattice expands strongly along the bSC and cSC directions and contracts by a comparable amount along aSC—together this results in a volume expansion reaching about 1% at the saddle-point configurations and decreasing again at even larger strains. The volume expansion is coupled to a strong increase in energy. Qualitatively, the relaxation pattern is the same for both shear systems, but the variation in the lattice constants is much larger under 兵211其具111典 shear while the symmetry remains at least monoclinic at all strains. At the saddle points we find that both lattice constants and angles agree with a bct structure, as shown in Fig. 7. In the saddle-point configurations the monoclinic and triclinic lattices of the 兵211其具111典 and 兵110其具111典 shear systems adopt tetragonal symmetry, the lattice constants correspond exactly to those determined along the PTP under uniaxial tension 共which is just rotated with respect to the bct saddle-point structure reached along the SOP兲. The most striking feature, however, is the strongly asymmetric character of the stress-strain curve. Due to the low value of the shear modulus, the stress increases very slowly, the stress-strain curve shows upward curvature. The G具111典 shear modulus derived from the initial slope of the stressstrain curve of V is G具111典 = 31.3⫾ 4 GPa, in reasonable agreement with the value derived from the elastic constants. As discussed above, energy and stress begin to increase at a

094108-8

PHYSICAL REVIEW B 81, 094108 共2010兲

ANOMALIES IN THE RESPONSE OF V, Nb, AND Ta TO… 0.20 ∆E = E(ε) - E(0) (eV/atom)

10

{110} {211}

bcc-V

bcc-V

8 6

0.15 σ31 (GPa)

4

0.10

2 0 -2 -4

0.05

-6 {110} {211}

-8

0.00

-10

0.0

0.1

0.2 0.3 Strain

2.65 2.60 2.55 2.50 2.45 2.40 4.50

0.0

0.1

(b)

0.2 0.3 Strain

0.4

0.5

bcc-V {110}

2.50

4.30

bSC=b

4.20 7.80 7.60 7.40 7.20 7.00

aSC

2.40 8.00 7.80 7.60 7.40 7.20

Lattice parameters (A)

4.40

bSC

4.70 4.50 4.30

cSC

cSC

4.10

90

αSC βSC γSC β

80 70 0.0

0.1

0.2

0.3 Strain

110 100 90 αSC βSC γSC

80 70 60

0.4

0.5

(d)

Angle (degree)

100

0.0

0.1

0.2

0.3 Strain

0.4

2.70 2.60 2.50 2.40 2.30 2.20 4.70

bcc-V {110} a c b

4.50 4.30 4.10

120 Angle (degree)

Angle (degree)

0.5

2.60 aSC=a c

110

(c)

0.4

2.70

bcc-V {211}

Lattice parameters (A)

Lattice parameters (A)

(a)

0.5

(e)

115 110 105 100 95 90 85 80 75

α β γ

0.0

0.1

0.2

0.3

0.4

0.5

Strain

FIG. 8. Variation in 共a兲 the total energy, 共b兲 the stress, 共c兲–共d兲 the lattice constants and angles of the computational super-cell, and 共e兲 of the distorted body-centered cell for bcc V as a function of the applied strain under 兵110其具111典 and 兵211其具111典 shear deformations.

strain large enough such that a pure shear deformation is insufficient to relax all lateral stresses and an expansion of the volume takes place. For both shear systems, the stress maximum is reached at a failure strain of about 0.2—this value is much larger than half of the strain at which the saddle point is located. The ideal tensile strength is 6.5 GPa for shearing along the 兵110其 and 5.5 GPa along the 兵211其 planes, the reduced shear strengths are 0.20 and 0.17, respectively 共see Table III兲. This means that the reduced shear strength is much higher than for Mo and W, although the actual shear strength reaches not even half this value. Nb shows a behavior under shear which is very similar to that discussed above for V. From the initial slope of the stress-strain curve we calculate a shear modulus of G具111典 ⬃ 22⫾ 4 GPa, in good agreement with the elastic constants. A remarkable difference is that the initial contraction of the lattice constant cSC at smaller strains has almost disappeared, and that aSC begins to shrink already at smaller strains. But again we observe a distinct change in the relaxation mode at a strain of ␥ ⬃ 0.08, slightly below the inflection point on the stress-strain curve. At larger strains, relaxation leads to a substantial volume expansion reaching 2% at the saddlepoint configuration. The saddle-point structures assumed at ␥ ⬃ 0.33 共for 兵211其具111典 shear兲 and ␥ ⬃ 0.29 共for 兵110其具111典 shear兲 are bct and agree with those assumed on the SOP under uniaxial 关100兴 tension 共cf. Figs. 9 and 4兲. The maximum shear stress is 6.0 GPa 共at a failure strain of ␥c = 0.2兲 for shearing parallel to the 兵211其 plane, and 7.8 GPa 共at ␥c

= 0.2兲 for shearing along 兵110其. These values are in good agreement with those of Luo et al.,21 although we find a slightly larger difference between both shear systems. The reduced value of the ideal shear strength is even larger than for V. For Ta the initial slope of the stress-strain curve yields G具111典 ⬃ 58⫾ 1 GPa in excellent agreement with the elastic constants. Only very modest relaxations are observed up to strains of about 0.1. Beyond this point, the lattice constant cSC increases strongly with increasing strain, while bSC and aSC undergo only a more modest expansion and contraction, respectively. These relaxations are also associated with an increasing volume expansion reaching 2% at the saddle point. The saddle-point configurations are reached at ␥ = 0.29 共for 兵110其具111典 shear兲 and ␥ = 0.32 共for 兵211其具111典 shear兲. The bct lattice constants of the saddle-point structures are a = c = 2.795 Å and b = 4.769 Å 共for 兵211其具111典 shear, those for 共110兲关111兴 shear agree within 0.01 Å兲, to be compared with a = 4.781 Å, b = c = 2.792 Å calculated along the PTP under uniaxial tension. The values of the ideal shear strength are 7.1 共6.5兲 GPa, at critical strains of ␥c = 0.22共0.20兲 for shearing parallel to the 兵110其 共兵211其 planes兲, respectively 共see Table III兲. Although they are much lower than those for Mo and W, all three metals show the same reduced shear strength. Hence for Ta the low value of the ideal shear strength is exactly as expected from the soft elastic shear modulus, while for V and Nb the extremely low shear modulus is not reflected by a similarly low value of the ideal shear strength.

094108-9

PHYSICAL REVIEW B 81, 094108 共2010兲

NAGASAKO et al. 0.20

10 8

0.15 σ31 (GPa)

4

0.10

-6

{110} {211} 0.0

0.1

0.2

bcc-Nb {211} aSC=a c

Lattice parameters (A)

0.4

0.5

0.0

bSC=b

cSC

0.1

(b)

2.90 2.85 2.80 2.75 2.70 8.80 8.60 8.40 8.20 8.00

0.2 0.3 Strain

Angle (degree)

90

αSC βSC γSC β

80 70 0.0

0.1

0.2

0.3 Strain

bSC

5.40 5.20 5.00 4.80 4.60

cSC

110 100 90 αSC βSC γSC

80 70 60

0.4

0.5

(d)

0.5

aSC

120

100

0.4

bcc-Nb {110}

Angle (degree)

Lattice parameters (A) Angle (degree)

0.3

{110} {211}

-8 -10

Strain

110

(c)

0 -2 -4

(a)

9.00 8.80 8.60 8.40 8.20 8.00

2

0.05

0.00

2.90 2.85 2.80 2.75 2.70 5.00 4.90 4.80 4.70 4.60

bcc-Nb

6

Lattice parameters (A)

∆E = E(ε) - E(0) (eV/atom)

bcc-Nb

0.0

0.1

0.2

0.3 Strain

0.4

0.5

(e)

2.90 2.85 2.80 2.75 2.70 5.00 4.90 4.80 4.70 4.60

bcc-Nb {110} a c b

115 110 105 100 95 90 85 80 75

α β γ

0.0

0.1

0.2

0.3

0.4

0.5

Strain

FIG. 9. Variation in 共a兲 the total energy, 共b兲 the stress, 共c兲–共d兲 the lattice constants and angles of the computational super-cell and 共e兲 of the distorted body-centered cell for Nb as a function of the applied strain under 兵110其具111典 and 兵211其具111典 shear deformations. VI. DISCUSSION AND CONCLUSIONS

We have demonstrated using ab initio DFT calculations that the response of body-centered cubic V and Nb to tensile and shear loading differs substantially from that of other bcc transition metals such as Mo, W, and Fe, but also from that of the heaviest metal of the V group, Ta. For these metals the stress-strain curves under tension or shear display a symmetric sinusoidal shape, with a period determined by the nearest extremum on the deformation path. Under uniaxial 具100典 tension this is a maximum corresponding to a fcc structure adopted under volume conservation at the Bain strain of ⑀ = 冑3 2 − 1 ⬃ 0.26. For all types of shear along the 具111典 this is a bct structure formed under volume conservation at a shear strain of ␥ = 冑2 / 4 ⬃ 0.35, i.e., at half the “twinning” strain recovering the bcc structure. As the initial slope of the stressstrain curve is determined by the relaxed tensile and shear modulus, respectively, the ideal tensile and shear strengths obey the relations

max =

0.26 E具100典 = 0.08E具100典 ,

共3兲

max =

0.35 G具111典 = 0.11G具111典 .

共4兲

For Mo and W the calculated moduli and ideal strength obey these relations with good accuracy. For V and Nb we

find that under uniaxial 具100典 loading a bifurcation from the primary tetragonal to a secondary orthorhombic deformation path occurs before reaching the stress maximum, strongly limiting the ideal tensile strength. Due to a shear instability, an orthorhombic deformation can occur under purely uniaxial load. It is interesting to correlate this shear instability induced by uniaxial strain to the softening of c44 under homogeneous compression. It has been shown that for V c44 vanishes at a pressure of about 60 GPa, leading to bcc → rhombohedral structural transition21,41,42,44 and that this phase transition is associated with the nesting properties of the Fermi surface and an electronic topological transition. While the homogeneous compression of the bcc lattice merely changes the nesting vector, a uniaxial strain changes the symmetry and therefore the topology of the Fermi surface. The saddle-point structure along the SOP is a special bct structure which can be made to coincide with the fct local energy minimum along the PTP by a rigid rotation and which is also identical to the saddle-point structure under shear deformation. For Ta the bifurcation to the SOP coincides with the stress-maximum along the PTP 共as has also been found for Mo兲. Because the ideal tensile strength is reached at a shear-unstable configuration, Ta fails under uniaxial loading not by cleavage, but by shear. The stress/tensile-strain curves of all three metals are strongly asymmetric along the PTP, but less so along the SOP. This means that the reduced tensile shear strength 쐓 = max / E具100典 is about 0.07 to 0.09, only

094108-10

PHYSICAL REVIEW B 81, 094108 共2010兲

ANOMALIES IN THE RESPONSE OF V, Nb, AND Ta TO… 0.20

10 8

0.15 σ31 (GPa)

4

0.10

-6

{110} {211} 0.0

0.1

0.2

bcc-Ta {211} aSC=a c

Lattice parameters (A)

0.4

0.5

0.0

bSC=b

cSC

0.1

(b)

2.90 2.85 2.80 2.75 2.70 8.80 8.60 8.40 8.20 8.00

0.2 0.3 Strain

0.4

aSC 2.90

bSC

5.40 5.20 5.00 4.80 4.60

cSC

Angle (degree)

90

αSC βSC γSC β

80 70 0.0

0.1

0.2

0.3

110 100 90 αSC βSC γSC

80 70 60

0.4

0.5

Strain

(d)

0.0

0.1

0.2

0.3

0.4

bcc-Ta {110}

2.85 2.80 2.75 4.90

a c b

4.80 4.70 4.60

120

100

0.5

bcc-Ta {110}

Angle (degree)

Lattice parameters (A) Angle (degree)

0.3

{110} {211}

-8 -10

Strain

110

(c)

0 -2 -4

(a)

9.00 8.80 8.60 8.40 8.20 8.00

2

0.05

0.00

2.90 2.85 2.80 2.75 2.70 5.00 4.90 4.80 4.70 4.60

bcc-Ta

6

Lattice parameters (A)

∆E = E(ε) - E(0) (eV/atom)

bcc-Ta

0.5

Strain

(e)

115 110 105 100 95 90 85 80 75

α β γ

0.0

0.1

0.2

0.3

0.4

0.5

Strain

FIG. 10. Variation in 共a兲 the total energy, 共b兲 the stress, 共c兲–共d兲 the lattice constants and angles of the computational super-cell, and 共e兲 of the distorted body-centered cell for Ta as a function of the applied strain under 兵110其具111典 and 兵211其具111典 shear deformations.

slightly larger than for Mo and W, although the ITS is determined by a different saddle-point configuration. Ta is a special case where the bifurcation point coincides with the inflection point on the PTP energy-strain curve. Hence the tetragonal stress maximum is reached at a shear-unstable configuration. Shearing bcc V or Nb in the 具111典 direction parallel to a 兵110其 or 兵211其 planes leads to strongly asymmetric stressstrain curves. A volume conserving unrelaxed 兵211其具111典 shear recovers the bcc structure at a strain of ␥ = 冑2 / 2, hence by symmetry the saddle-point configuration should fall at ␥ ⬃ 0.35 and the inflection point or stress maximum at ␥c

⬃ 0.175. However, due to a very low relaxed shear modulus G关111兴, the initial slope of the stress-strain curve is very low. The stress begins to increase strongly at ␥ ⬃ 0.08 were the relaxation pattern changes qualitatively, accompanied by an incipient volume expansion. The saddle-point structure for both glide systems has bct symmetry, it is reached at strains between 0.28 and 0.32 depending on the glide plane. For 兵110其具111典 shear a strong relaxation is required to reach this configuration. This bct saddle-point structure is the same as that reached on the SOP under uniaxial 具100典 tension. For V the failure strain is ␥c = 0.20, the ideal shear strength is 6.5 and 5.5 GPa for the 兵110其 and 兵211其 glide planes, respec-

TABLE III. Ideal shear strengths max, critical strain ␥c, shear modulus G关111兴 of V, Nb, and Ta under uniaxial 关100兴 loading, as determined by the stress maximum along the tetragonal and orthorhombic deformation paths. 兵110其具111典

V Nb Ta Mo W

This work This work Ref. 21 This work Ref. 21 Ref. 19

兵211其具111典

G具111典

max

␥c

max / G具111典

max

␥c

max / G具111典

33 31

6.54 7.8 7.6 7.1 16.1 18.2

0.21 0.20 0.22 0.22 0.17 0.17

0.20 0.25

5.5 6.0 6.4 6.5 15.8 18.1

0.21 0.20 0.20 0.201 0.17 0.17

0.17 0.19

53 134 163

094108-11

0.13 0.12 0.11

0.12 0.12 0.11

PHYSICAL REVIEW B 81, 094108 共2010兲

NAGASAKO et al.

tively. The reduced shear strengths are 쐓 = 0.20 and 0.17— i.e., nearly twice as high as expected for a symmetric stressstrain curve and as calculated for Mo and W. Nb follows the same pattern, with an even slightly larger reduced shear strength. In summary: 共i兲 For both V and Nb the ideal tensile strength under 具111典 loading is limited by a bifurcation to an orthorhombic deformation path, but it is still about twice as large as the ideal shear strength for shearing in the 具111典. 共ii兲 The stress-strain curves for V and Nb under shear deformation are strongly asymmetric, the ideal shear strength is much higher than expected on the basis of a very low shear modulus. This reflects an increasing stiffness of the lattice under increasing shear strain, as shown by the relaxation behavior. 共iii兲 The saddle-point configurations reached under tensile and shear loading have the same special bct structure. For this reason and because the ideal shear strength is much lower than the tensile strength, both metals will fail by shear and not by cleavage. 共iv兲 The response of Ta to tensile and shear loading is more similar to that of Mo or W. However, because the stress maximum under tension is reached at a shear-unstable configuration, Ta will also fail by shear and not by cleavage.

*[email protected] †[email protected]

ACKNOWLEDGMENTS

Work at the University of Vienna has been supported by the VASP project and within the University Research Focus “Material Science” and “Computational Science.” We thank T. Bučko for provision of GADGET structural optimization package.

Philos. Mag. A 81, 1725 共2001兲. R. Krenn, D. Roundy, J. W. Morris, Jr., and M. L. Cohen, Mater. Sci. Eng., A 319-321, 111 共2001兲. 21 W. Luo, D. Roundy, M. L. Cohen, and J. W. Morris, Jr., Phys. Rev. B 66, 094110 共2002兲. 22 M. Jahnátek, M. Krajčí, and J. Hafner, Philos. Mag. 87, 1769 共2007兲. 23 M. Jahnátek, M. Krajčí, and J. Hafner, Phys. Rev. B 76, 014110 共2007兲. 24 M. Jahnátek, J. Hafner, and M. Krajčí, Phys. Rev. B 79, 224103 共2009兲. 25 J. Pokluda, M. Černy, P. Šandera, and M. Šob, J. Comput.-Aided Mater. Des. 11, 1 共2004兲. 26 D. M. Clatterbuck, C. R. Krenn, M. L. Cohen, and J. W. Morris, Jr., Phys. Rev. Lett. 91, 135501 共2003兲. 27 H. Kitagawa and S. Ogata, Key Eng. Mater. 161-163, 443 共1999兲. 28 S. Ogata and S. Yip, Science 298, 807 共2002兲. 29 S. Ogata, J. Li, and S. Yip, Phys. Rev. B 71, 224102 共2005兲. 30 M. Černy, M. Šob, J. Pokluda, and P. J. Šandera, J. Phys.: Condens. Matter 16, 1045 共2004兲. 31 M. Šob, L. G. Wang, and V. Vitek, Kovove Mater. 36, 145 共1998兲. 32 D. M. Clatterbuck, D. C. Chrzan, and J. W. Morris, Jr., Acta Mater. 51, 2271 共2003兲. 33 M. Friák, M. Šob, and V. Vitek, Philos. Mag. A 83, 3529 共2003兲. 34 M. Jahnátek, M. Krajčí, and J. Hafner, 共unpublished兲. 35 W. Luo, M. L. Cohen, and J. W. Morris, Jr., Philos. Mag. Lett. 89, 23 共2009兲. 36 J. Trivisonno, S. Vatanayon, M. Wilt, J. Washick, and R. Reifenberger, J. Low Temp. Phys. 12, 153 共1973兲. 37 K. W. Katahara, M. H. Manghnani, and E. Fisher, J. Phys. F: Met. Phys. 9, 773 共1979兲. 20 C.

‡[email protected] §

For Ta the ideal shear strength found in our calculations 关max = 7.1共6.5兲 GPa for 兵110其具111典 and 兵211其具111典 shear兴 is in excellent agreement with experimental estimates based on nanoindentation measurements4 yielding an ideal shear strength of about 7.5 GPa. From the nanoindentation experiments and experimental observations of plastic flow response to large strain impact testing62 it was also suggested the 兵110其具111典 slip system is preferred over the 兵211其具111典 slip system, but we find only very small differences in the limiting shear strengths and in the critical strains. However, it is certainly encouraging to see that experimental and theoretical determinations of the ideal strength of metals begin to converge.

[email protected] 1 A. Kelly and N. H. MacMillan, Strong Solids, 3rd ed. 共Clarendon Press, Oxford, 1986兲. 2 N. Gane and F. P. Bowden, J. Appl. Phys. 39, 1432 共1968兲. 3 S. G. Corcoran, R. J. Colton, E. T. Lilleodden, and W. W. Gerberich, Phys. Rev. B 55, R16057 共1997兲. 4 M. M. Biener, J. Biener, A. M. Hodge, and A. V. Hamza, Phys. Rev. B 76, 165422 共2007兲. 5 C. A. Schuh, J. K. Mason, and A. C. Lund, Nature Mater. 4, 617 共2005兲. 6 C. A. Schuh, Mater. Today 9, 32 共2006兲. 7 J. Frenkel, Z. Phys. 37, 572 共1926兲. 8 R. Hill and F. Milstein, Phys. Rev. B 15, 3087 共1977兲. 9 F. Milstein and K. Huang, Phys. Rev. B 18, 2529 共1978兲. 10 F. Milstein and B. Farber, Phys. Rev. Lett. 44, 277 共1980兲. 11 F. Milstein, J. Marschall, and H. E. Fang, Phys. Rev. Lett. 74, 2977 共1995兲. 12 F. Milstein and S. Chantasiriwan, Phys. Rev. B 58, 6006 共1998兲. 13 A. T. Paxton, P. Gumbsch, and M. Methfessel, Philos. Mag. Lett. 63, 267 共1991兲. 14 W. Xu and J. A. Moriarty, Phys. Rev. B 54, 6941 共1996兲. 15 P. Alippi, P. M. Marcus, and M. Scheffler, Phys. Rev. Lett. 78, 3892 共1997兲. 16 M. Šob, L. G. Wang, and V. Vitek, Mater. Sci. Eng., A 234-236, 1075 共1997兲. 17 M. Šob, L. G. Wang, and V. Vitek, Philos. Mag. B 78, 653 共1998兲. 18 D. Roundy, C. R. Krenn, M. L. Cohen, and J. W. Morris, Jr., Phys. Rev. Lett. 82, 2713 共1999兲. 19 D. Roundy, C. R. Krenn, M. L. Cohen, and J. W. Morris, Jr.,

094108-12

PHYSICAL REVIEW B 81, 094108 共2010兲

ANOMALIES IN THE RESPONSE OF V, Nb, AND Ta TO… 38

H. Kojima, M. Shino, and T. Suzuki, Acta Metall. 35, 891 共1987兲. 39 F. H. Featherston and J. R. Neighbours, Phys. Rev. 130, 1324 共1963兲. 40 K. W. Katahara, M. H. Manghnani, and E. Fisher, J. Appl. Phys. 47, 434 共1976兲. 41 A. Landa, J. Klepeis, P. Söderlind, I. Naumov, O. Velikokhatnyi, L. Vitos, and A. Ruban, J. Phys.: Condens. Matter 18, 5079 共2006兲. 42 L. Koči, Y. Ma, A. R. Oganov, P. Souvatzis, and R. Ahuja, Phys. Rev. B 77, 214101 共2008兲. 43 P. Söderlind, O. Eriksson, J. M. Wills, and A. M. Boring, Phys. Rev. B 48, 5844 共1993兲. 44 Y. Ding, R. Ahuja, J. Shu, P. Chow, W. Luo, and H. K. Mao, Phys. Rev. Lett. 98, 085502 共2007兲. 45 T. Kenichi and A. K. Singh, Phys. Rev. B 73, 224119 共2006兲. 46 Y. Nakagawa and A. D. B. Woods, Phys. Rev. Lett. 11, 271 共1963兲. 47 R. Colella and B. W. Batterman, Phys. Rev. B 1, 3913 共1970兲. 48 W. Luo, R. Ahuja, Y. Ding, and H. Mao, Proc. Natl. Acad. Sci. U.S.A. 104, 16428 共2007兲. 49 C. M. Varma and W. Weber, Phys. Rev. B 19, 6142 共1979兲.

G. Kresse and J. Furthmüller, Comput. Mater. Sci. 6, 15 共1996兲. Kresse and J. Furthmüller, Phys. Rev. B 54, 11169 共1996兲. 52 J. P. Perdew, J. A. Chevary, S. H. Vosko, K. A. Jackson, M. R. Pederson, D. J. Singh, and C. Fiolhais, Phys. Rev. B 46, 6671 共1992兲. 53 P. E. Blöchl, Phys. Rev. B 50, 17953 共1994兲. 54 G. Kresse and D. Joubert, Phys. Rev. B 59, 1758 共1999兲. 55 T. Bučko, J. Hafner, and J. G. Ángyán, J. Chem. Phys. 122, 124508 共2005兲. 56 R. P. Feynman, Phys. Rev. 56, 340 共1939兲. 57 O. H. Nielsen and R. M. Martin, Phys. Rev. Lett. 50, 697 共1983兲. 58 H. J. Monkhorst and J. D. Pack, Phys. Rev. B 13, 5188 共1976兲. 59 M. Methfessel and A. T. Paxton, Phys. Rev. B 40, 3616 共1989兲. 60 P. E. Blöchl, O. Jepsen, and O. K. Andersen, Phys. Rev. B 49, 16223 共1994兲. 61 J. W. Morris, Jr., C. R. Krenn, D. Roundy, and M. L. Cohen, in Phase Transformations and Evolution in Materials, edited by P. E. Turchi and A. Gonis 共TMS, Warrendale, PA, 2000兲, p. 187. 62 P. J. Maudlin, J. F. Bingert, and G. T. Gray, Int. J. Plast. 19, 483 共2003兲. 50

51 G.

094108-13

Anomalies in the response of V, Nb, and Ta to tensile and shear loading: Ab initio density functional theory calculations Naoyuki Nagasako,1,* Michal Jahnátek,2,† Ryoji Asahi,1,‡ and Jürgen Hafner2,§ 1

Toyota Central Research and Development Laboratories Inc., Nagakute, Aichi 480-1192, Japan Faculty of Physics and Center for Computational Materials Science, University of Vienna, Sensengasse 8/12, A-1090 Wien, Austria 共Received 21 December 2009; revised manuscript received 9 February 2010; published 17 March 2010兲

2

Ab initio density functional calculations of the response of V, Nb, and Ta to tensile and shear loading have been performed. We find that the behavior of all three metals of the V group under large strains differs considerably from that reported for the other body-centered cubic 共bcc兲 transition metals 共Mo, W, and Fe兲. Under unaxial 具100典 tensile loading, V and Nb undergo a bifurcation from a tetragonal to an orthorhombic deformation path, associated with a shear instability, before reaching the stress maximum. The bifurcation strongly reduces the ideal tensile strengths to 11.5 GPa for V and 12.5 GPa for Nb. For Ta the bifurcation point coincides with the stress maximum of 13.6 GPa along the tetragonal path so that the metal fails under tensile strain by shear and not by cleavage. The stress-strain curves calculated for the 兵110其具111典 and 兵211其具111典 slip systems are strongly asymmetric; the ideal shear strengths for both slip systems are 6.5 共5.5兲 GPa for V and 7.8 共6.0兲 GPa for Nb. Hence the ideal shear strengths are only half as large as for the bcc metals Mo and W, but much larger than expected on the basis for the low shear moduli of V and Nb. Ta shows a behavior intermediate between these two groups of metals, with a calculated ideal shear strength of 7.1 共6.5兲 GPa, in excellent agreement with the experimental estimate from nanoindentation experiments. The saddle-point structure determining the shear strength for both slip systems is a special body-centered-tetragonal structure. This structure is identical to the saddle-point structure identified on the orthorhombic deformation path under uniaxial tension. Hence also V and Nb will fail under uniaxial tension not by cleavage, but by shear. DOI: 10.1103/PhysRevB.81.094108

PACS number共s兲: 61.72.Nn, 62.25.⫺g, 62.20.F⫺

I. INTRODUCTION

The strength of any solid is limited by the ideal or theoretical strength defined by the stress required to yield or break a perfect crystal. The ideal shear strength determines the stress necessary for the nucleation of dislocations, while for the formation of a cleavage crack the local stress must exceed the ideal tensile strength.1 In real solids the maximum attainable stress is strongly influenced by the formation of mobile dislocations, by grain boundaries, cracks, and other microstructural features, but it can never exceed the ideal value. While no experimental determinations of the ideal strength under tension have been possible to date, the ideal shear strength can be estimated from nanoindentation experiments.2–6 In nanoindentation experiments the indenter is so small that the volume of the probe undergoing shear deformation may be considered as defect free. In a typical nanoindentation test force and displacement are recorded as the indenter tip is pressed into the materials surface. The yield stress is identified by the first point at which the experimental data deviate from the elastic curve. At this point the indenter moves into the substrate without a measurable increase of the load—this is usually interpreted as a homogeneous dislocation nucleation event.5,6 However, a detailed analysis of the load/displacement curves and detailed molecular dynamics simulations suggest that the nominally “elastic” part of the curve might contain some superimposed plastic deformation too subtle to be detected. This would mean that even nanoindentation experiments can seriously underestimate the theoretical strength. For example, Biener et al.4 derived for body-centered cubic Ta a maximal shear stress of 7.5 GPa, considerably below the theoretical shear 1098-0121/2010/81共9兲/094108共13兲

strength of 11 GPa estimated from the shear modulus of 69 GPa. In view of the difficulty to determine the ideal strength in experiments, there is a continuing interest in its theoretical calculations. The earliest attempts assumed a simple analytic form of the stress-strain curve which allows to derive the ideal strength from the elastic moduli.1,7 This allows to define a dimensionless shear and tensile strength, 쐓 = max / E and 쐓 = max / G, where max and max are the maxima of tensile and shear stress and E and G are the experimental values of the Young’s modulus and the shear modulus for the direction of loading. The reduced dimensionless shear and tensile strengths are assumed to be essentially constant for a specific class of materials. A significant step forward was realized since the 1970s using atomistic models based on empirical or semiempirical force fields which provided valuable information on the atomistic mechanisms of the deformation under large strains.8–12 However, because the parameters of the force fields were necessarily fitted to the materials properties at small strains, the predictions cannot be considered as quantitatively reliable. Finally since the 1990s ab initio density functional calculations began to supercede empirical methods for the determination of the response of metals and intermetallic compounds to tensile and shear loading.13–24 These methods are free from adjustable parameters, valid at all strains and permit in principle a quantitative determination of the ideal strengths. However, because of the relatively large computational effort required in such calculations, early studies were performed at fixed strains.13,14 In this case the selected strain was stepwise increased by small increments while the other five independent strains were fixed at zero, i.e., all internal relaxations were suppressed.

094108-1

©2010 The American Physical Society

PHYSICAL REVIEW B 81, 094108 共2010兲

NAGASAKO et al.

More meaningful results for the energy-strain and stressstrain relations are achieved if the crystal is relaxed until only the stress conjugate to the applied strain has a nonzero value. A review of semiempirical and ab initio calculations of ideal tensile and shear strengths has recently been compiled by Pokluda et al.25 Even to date, ab initio calculations of tensile and shear strengths are available only for a few selected metals and for a very few intermetallic compounds. The face-centered cubic 共fcc兲 metals Al 共Refs. 18, 22–24, and 26–29兲 and Cu 共Refs. 18, 22–24, 30, and 31兲 have been studied most extensively. Among the body-centered cubic metals attention was focused on Fe 共Refs. 32 and 33兲 and on the refractory metals Mo and W.16,19,21 The studies of the fcc metals Al and Cu have emphasized that estimates of the ideal strength based on the elastic be¯ 典 and havior are of limited validity: for both 兵111其具112 ¯ 兵111其具110典 shear deformations, the shear constants of Cu are much higher than those of Al, while from the position of the maximum on the stress-strain curve a higher ideal shear strength is predicted for Al.24,28 The investigations of the loading behavior of the fcc metals have also demonstrated that the theoretical strength may be limited by a shear-related instability, by the softening of a phonon mode along a tensile deformation path or by stacking-fault formation along a shear deformation path, even before the maximum in the stress-strain curve has been reached. For example, the ideal tensile strength 共ITS兲 of Cu under 关100兴 loading is limited by the occurrence of a shear instability30,34 at a strain of 10%. The instability induces a bifurcation from a tetragonal to an orthorhombic deformation path and limits the ITS to 9.5 GPa, compared a stress maximum of 23.8 GPa at a strain of 36.0%. For Al Clatterbuck et al.26 have reported phonon instabilities under uniaxial 关100兴 tension at strains of 17% and 18% limiting the ITS to 9.2 GPa compared to a peak value of 12.9 GPa, under 关110兴 tension a soft phonon mode appears at a strain of 11%. In all cases the soft phonon modes show displacement patterns corresponding to periodic shear defor¯ 典 and 兵111其具1 ¯ 10典 shear mations. For Al under both 兵111其具112 deformations the ideal shear strength 共ISS兲 is limited by 共i兲 stacking fault instabilities and 共ii兲 soft phonon modes.24,26 ¯ 典 shear the unstable stacking fault configuUnder 兵111其具112 ration is reached at a strain of 14.5%, at the same strain a phonon instability has been reported. The displacement of ¯ 典 shear failthe soft phonon mode corresponds to 兵111其具112 ure with a periodicity of two or three 兵111其 planes, it is also closely related to the failure mode induced by the soft phonon mode predicted for 关110兴 tension 共for a detailed discussion we refer to Jahnátek et al.兲24 For fcc Cu, no shear instabilities occur under uniaxial 关110兴 or 关100兴 tensile loading. Also, in contrast to Al the unstable stacking fault configura¯ 典 and 兵111其具1 ¯ 10典 shear deformations tions under 兵111其具112 are reached only at strains beyond the maximum on the stress-strain curve.23,24,34 In comparison to this very complex scenario, the investigations of the bcc metals presented so far describe a much simpler picture. Investigations of tensile loading have concentrated on the 具100典 directions because symmetry

considerations,12 early ab initio calculations16 and empirical tests have all identified the 具100典 directions as the weak directions in tension and the 兵100其 planes as cleavage planes. The general theory of the response of cubic metals to uniaxial loading along 具100典 has been developed in a series of classical papers by Milstein et al.10,11 Starting from an unstressed bcc structure all metals first adopt a primary deformation path with tetragonal guiding symmetry. Any deviation from tetragonality implies the presence of a transverse load. However, as already shown by Hill and Milstein8 at a “special invariant state” where the elastic constants satisfy the condition c22 = c23, a bifurcation to a secondary orthorhombic path may occur under dead load 共note that the invariance condition implies a tetragonal shear instability兲. For the refractory bcc metals Mo and W 共Refs. 19 and 21兲 and for bcc Fe 共Ref. 32兲 it has been shown that the tetragonal symmetry is broken only after the point of maximum tensile stress has been passed. Only for bcc Nb the bifurcation occurs already at a lower strain and leads to an ITS which is significantly lower 共13.1 GPa兲 than that on the tetragonal path 共18.8 GPa兲. Shear deformations along 具111典 may occur in bcc crystals by slip on the 共110兲, 共112兲, and 共123兲 planes. All three shear systems have been studied by Roundy et al.19 for W, while for Mo, Nb, and Fe only the two first have been investigated. The stress-strain curves are very similar for 关111兴 slip along all investigated glide planes, leading to similar values of the ISS. A remarkable result is that for all bcc metals with the exception of Nb the reduced dimensionless tensile and shear strengths are very close to the ideal values, 쐓 = max / E = 0.08 and 쐓 = max / G = 0.11, calculated under the assumption of a sinusoidal stress-strain curve with a period that is twice the strain required to reach the saddle-point structure determining the ideal strength 共i.e., the fcc phase in tension and a body-centered tetragonal phase under shear兲. The stress-strain curve of Nb under shear shows a strong deviation with a low initial slope caused by a low shear modulus, the reduced ideal shear strength is 쐓 = 0.18, i.e., 50% higher than for the other bcc metals. Together these results show that among all investigated bcc metals Nb is the only one that is predicted to fail by 兵211其具111典 shear rather than by 关100兴 tensile failure. In very recent work35 the effect of a superposed transverse stress has been considered. As observed for other metals, hydrostatic tension raises, while hydrostatic compression lowers the ITS of Nb. The exceptional behavior of Nb under tensile and shear loading has been attributed to a very low G具111典 / E具100典 ratio were the relaxed modulus for 关100兴 tension is given by E具100典 =

共c11 − c12兲共c11 + 2c12兲 , c11 + c12

共1兲

3c44共c11 − c12兲 , 4c44 + c11 − c12

共2兲

and G具111典 =

is the relaxed modulus for shear along 具111典 共note that because of the threefold rotational symmetry around the 具111典 axes, any shear in this direction has the same modulus兲. Using the experimental values of the elastic constants36–40 this

094108-2

PHYSICAL REVIEW B 81, 094108 共2010兲

ANOMALIES IN THE RESPONSE OF V, Nb, AND Ta TO…

ratio is G / E = 0.34, 0.28, and 0.42 for V, Nb, and Ta, and G / E = 0.35 and 0.39 for Mo and W. This would suggest that the anomalous behavior under tensile and shear loading should be restricted to Nb, while V and Ta should be expected to behave similarly as Mo and W. However, it is well known that Nb and V share some interesting anomalies in their elastic, dynamic, and superconducting properties: 共i兲 low values of the trigonal and tetragonal shear constants 共c44 = 43, 29, and 83 GPa for V, Nb, and Ta; c⬘ = 共c11 − c12兲 / 2 = 55.5, 57 and 53 GPa for V, Nb, and Ta兲. 共ii兲 Theoretical calculations41,42 predict a pronounced softening of the trigonal shear modulus of V and Nb under compression, driving a mechanical instability of bcc V while for Nb the shear modulus softens for pressures around 50 GPa, but remains positive. The occurrence of a structural phase transition of V from bcc to a rhombohedral phase at about 63–69 GPa has recently been confirmed by synchrotron x-ray diffraction.44 In contrast the absence of pressure-induced phase transitions in Nb up to 145 GPa has recently been confirmed.45 共iii兲 The elastic anomalies of V and Nb are reflected in anomalies of their phonon dispersion relations.46–48 共iv兲 Phonon softening is thought to be responsible for the high superconducting transition temperature Tc in Nb and for the strong increase of Tc under compression in V. The elastic and phonon anomalies have been discussed extensively in relation to the electronic properties and shown to be related to the nesting properties of the Fermi surface.42,49 In particular, the downward dispersion of the transverse phonon branch along 关100兴 and therefore also the unusual softness of c44 has been shown to arise from the nesting properties of the Fermi surface around the N point leading to a van Hove singularity in the electronic density of states close to the Fermi energy. Here we present an extended study of the response of all three V-group metals to tensile and shear loading based on ab initio density functional calculations. Our calculations allow for a bifurcation from a tetragonal to an orthorhombic deformation path under uniaxial tensile strain. Shear deformations have been studied for the 兵110其具111典 and 兵211其具111典 shear systems.

The crystal structure was fully relaxed at each deformation step until all lateral stresses vanished. This has been done by the efficient external optimizer GADGET developed by Bučko et al.55 GADGET performs a relaxation in terms of generalized coordinates which allow a better control of lateral stresses. The forces acting on the atoms were computed via the Hellmann-Feynman theorem,56 the stress tensor acting on the unit cell was computed via the generalized virial theorem.57 The use of a high cut-off energy allows to achieve a high accuracy of the components of the stress tensor. The Brillouin zone 共BZ兲 was sampled using various types of meshes according to the size and symmetry of the computational cells. Because the elastic properties and the stresses at small strains of V and Nb are strongly influenced by the occurrence of van Hove anomalies close to the Fermi level, very fine k-point meshes 共up to 23⫻ 23⫻ 23 for calculations based on a simple face-centered or body-centered tetragonal cell and up to 22⫻ 14⫻ 8 for the larger supercells used for simulating shear deformations兲 are required to calculate the elastic shear constants and the stress-strain relations. All integration meshes were constructed according to the Monkhorst-Pack scheme.58 The integration over the BZ used the Methfessel-Paxton method59 with the smearing parameter of 0.2 eV for calculation of the total energies and stresses, and the tetrahedron method with Blöchl corrections60 for the calculation of the density of states. The total energy was calculated with high precision, converged to 10−8 eV/ atom. The structural relaxation was stopped when all forces acting on the atoms where converged to within 10−3 eV/ Å and all components of the stress tensor except that conjugate to the imposed strain where converged to within 0.05 GPa. For the calculation of the elastic constants we used the linear-interpolation method of the stress tensors. The cubic cells were submitted to the ⫾1 and ⫾4 strains; the tetragonal cells were submitted in addition to ⫾3 and ⫾6 strains; for the orthorhombic cells two more strains, ⫾2 and 5; were added. For each set of strains ⫾i two different magnitudes of 0.2% and 0.5% were used. For the calculation of the elastic constants the total energy was calculated with even higher accuracy, converged to 10−9 eV/ atom.

II. COMPUTATIONAL METHODS

III. ELASTIC PROPERTIES

Our ab initio total-energy and force calculations are based on density functional theory 共DFT兲 as implemented in the Vienna ab initio simulation package 共VASP兲.50,51 A gradientcorrected functional has been used to describe electronic exchange and correlations.52 Electron-ion interactions are treated within the projector-augmented wave 共PAW兲 method.53,54 For all elements we used the standard PAW pseudopotentials 共PP兲 distributed with VASP with reference configurations np6nd4共n + 1兲s1 for the valence states with n = 3 , 4, and 5 for V, Nb, and Ta. The plane-wave basis set contained components with kinetic energies up to 350 eV. The response of the crystal to tensile or shear deformations was calculated by increasing the strain along the chosen directions in small steps. Increasing/decreasing the strain by very small increments leads to a reversible deformation process at zero absolute temperature with negligible hysteresis.

The elastic constants of the V-group metals, together with the Young’s modulus E具100典 for tension along 具100典 and the relaxed shear modulus G具111典 for shear along the 具111典 direction are compiled in Table I. It is well known that although very good agreement for the bulk modulus 关B = 共c11 + 2c12兲 / 3兴 and the orthorhombic shear constant c⬘ = 共c11 − c12兲 / 2 is achieved, all DFT calculations seriously underestimate the trigonal shear constant c44, irrespective of the exchange-correlation functional 共local or semilocal gradientcorrected functional兲 and of the method used for solving the Kohn-Sham equations 共plane-wave based pseudopotential or PAW calculations, muffin-tin orbital methods兲.41–43 The low value of the trigonal shear constant is related to an anomalous dispersion of transverse acoustic phonons propagating along the 具100典 direction. In the long-wavelength limit, shear constant, and frequencies of transverse acoustic phonons are

094108-3

PHYSICAL REVIEW B 81, 094108 共2010兲

NAGASAKO et al.

TABLE I. Elastic constants, shear anisotropy A = 2共c⬘ − c44兲 / c44, relaxed tensile modulus E具100典, relaxed shear modulus G具111典, and ratio G/E for the body-centered cubic metals of the V group 共in GPa兲. Metal V

Nb

Ta

Mo

W

Reference

c11

c12

c44

c⬘ = 共c11 − c12兲 / 2

A

E具100典

G具111典

G/E

This work Theory, Ref. 42 Theory, Ref. 43 Exp., Ref. 37 This work Theory, Ref. 42 Theory, Ref. 43 Exp., Ref. 37 This work Theory, Ref. 42 Theory, Ref. 43 Exp., Ref. 37 This work Theory, Ref. 43 Exp., Ref. 37 This work Theory, Ref. 43 Exp., Ref. 37

262 260 205 231 247 247 267 246 257 265 291 266 470 406 465 500 553 523

144 135 130 120 138 138 147 133 163 159 162 161 161 150 162 205 207 204

17 17 5 43 17 10 27 29 71 74 84 83 105 107 109 130 178 161

59 63 37.5 55.5 54.5 54.5 60 57 47 53 64.5 53 154 128 152 148 173 159

4.9 5.4 13.0 0.56 4.4 8.9 2.4 1.9 −0.68 −0.57 −0.46 −0.72 0.93 0.40 0.78 0.27 −0.06 0.03

160 168 104 149 148 148 163 154 132 146 175 145 386 325 381 382 440 407

32 33 12 50 31 22 43 43 53 59 70 60 133 120 134 142 175 159

0.20 0.20 0.11 0.33 0.21 0.15 0.26 0.28 0.40 0.40 0.40 0.41 0.34 0.37 0.35 0.37 0.40 0.39

related through c44 = 2共q兲 / q2 where is the density. Softening of acoustic phonons and the low value of the shear constant are related to the nesting properties of the Fermi surface which produce a van Hove singularity in the electronic density of states 共DOS兲 close to the Fermi level, as discussed in detail by Landa et al.41 As shown in Fig. 1, the distance between the van-Hove peak in the DOS and the Fermi energy increases from V to Nb and Ta, in correspondence to an increasing value of the shear constant. Due to the presence of the van-Hove singularity, an exact determination of c44 requires a very fine mesh for Brillouin zone integrations. With a 23⫻ 23⫻ 23 grid, full convergence is achieved, but the shear constant is still too low by a factor of about two. It is well known that crystalline imperfections tend to smear out the Fermi surface and hence the singularity in the DOS and that this results in a damping of the related anoma-

Total DOS (states/eV/cell)

3.5

bcc-V bcc-Nb bcc-Ta

3.0

lies in the phonon dispersion relations and to a stiffening of the elastic shear modes. In theoretical calculations this effect may be modeled by applying a Gaussian smearing to the eigenstates and we find that a broadening of the energy levels leads to a larger value of the c44 shear constant. While this might account for part of the discrepancy between theory and experiment, more accurate experiments at low temperatures and high-quality specimens would also be desirable. For the moment we note that the very low values resulting from all theoretical calculations should be treated with caution, although the trends among the V-group metals are at least semiquantitatively correct. We also note that for the relaxed tensile and shear moduli relevant to the present study, agreement between theory and experiment is better than for c44 alone. To assess the validity of our method for calculating the elastic constants of bcc transition metals we include in Table I our results for Mo and W, together with the experimental values. For both metals we note very good agreement between theory and experiment.

2.5

IV. RESPONSE TO UNIAXIAL [100] TENSILE LOADING

2.0 1.5 1.0 0.5 0.0 -8

-6

-4

-2

0

2

Energy (eV)

FIG. 1. 共Color online兲 Electronic density of states of bcc V, Nb, and Ta. Note the van-Hove singularities close to the Fermi level.

The general theory of the response of cubic metals to uniaxial 具100典 loading has been formulated by Milstein et al.8,9,11 On the primary tetragonal deformation path 共the Bain path兲 the structure can be considered as either body-centered tetragonal 共bct兲 or face-centered tetragonal 共fct兲. By symmetry only three stress-free states are possible: bcc, fcc, and a special bct 共or equivalently fct兲 structure, but the order of appearance of these states along the deformation path depends on the details of interatomic binding. Owing to crystal symmetry, the fcc state can be reached from the bcc state

094108-4

PHYSICAL REVIEW B 81, 094108 共2010兲

ANOMALIES IN THE RESPONSE OF V, Nb, AND Ta TO… a2 = c

fcc

0.40

fct

a1 = b1 = a

Tetragonal path a3 = 2 a ′ 2

b3 = a′

b2 = a′

a3 = c

(b) Saddle-point structure ~ y y a3 = a0 ~ z

a1 = b1 = a0

(c) Structure at local energy-minimum

b2 = 2a0

(a) Unstrained structure Orthorhombic path

bct

c

0.20 0.15 0.10 0.05 0.00

b3 = 2a0

z

b2 = 2c

b3 = 2c

bcc

fct

a0

a0 b1 = 2c

c b3 = 2c b2 = a (d) Saddle-point structure

bcc-V

-0.05

fct

0.0

(a)

0.1

0.2 0.3 Strain

b1 = 2a0

0.4

b3 = a0

(e) Structure at energy-minimum

only by applying uniaxial tension, hence there are three possible orderings of the stress-free states: 共1兲 bcc, bct, fcc 共as found for the alkali metals兲,11 共2兲 bct, bcc, fcc, and 共3兲 bcc, fcc, bct. The centrally located stress-free state is necessarily unstable because of a decreasing stress at increasing strain, it represents a saddle point on the energy-strain curve. Scenario 共3兲 is realized along the tetragonal deformation path of the bcc transition metals such as W.18–20 If the primary tetragonal path 共PTP兲 contains the “special invariant state” where c22 = c23, a bifurcation to a secondary orthorhombic path 共SOP兲 can occur under strict uniaxial load. Immediately after bifurcation the system passes through a stress-free bct state while at larger strain the original bcc structure is recovered. Figure 2共a兲 shows a sketch of the bcc lattice embedded into a more general fct lattice. Tetragonal deformations can be described by the variation of the lattice parameters a1 and a2 = a3 of a bct lattice with a1 increasing linearly as a function of strain. The deformations along an orthorhombic deformation path can be described in terms of a fct lattice with b1 = a1 = a0 and b2 = b3 = 冑2a0 in the undeformed state. Along the PTP relaxation minimizes the total energy with respect to a2 = a3 only, while along the SOP the total energy is minimized independently with respect to both b2 and b3. The energy-strain and stress-strain curves, as well as the variation in the lattice parameters ai and bi as a function of strain are shown for V, Nb, and Ta in Figs. 3–5. As a measure of strain we use the engineering strain. The scenario is qualitatively the same for all three metals, albeit with some important quantitative differences. Along the PTP the maximum on the energy-strain curve is the fcc structure as shown in Fig. 2共b兲. Under a volume-conserving deformation the strain at which the bct cell assumes the fcc structure is given by the Bain strain of ⑀B = 冑3 2 − 1 = 0.26. For all three metals the fcc structure is realized at a slightly larger strain varying from ⑀ = 0.274 for V to ⑀ = 0.273 for Nb and ⑀ = 0.271 for Ta,

Orthorhombic path Tetragonal path

bcc-V 0.0

(b)

0.1

0.2 0.3 Strain

0.4

0.5

bcc-V

5.0

FIG. 2. 共Color online兲 Sketch of the PTP and SOP deformation paths of a body-centered cubic lattice shown in red 共black兲 under uniaxial 关100兴 tensile loading. The structures along the PTP are described within the body-centered tetragonal reference frame 共lattice constants ai , i = 1 – 3兲, those along the SOP are described as face-centered tetragonal 关shown in blue 共gray兲—lattice constants bi , i = 1 – 3兴.

30 25 20 15 10 5 0 -5 -10 -15 -20 -25 -30

5.5

a0 b2 = 2a0

0.5

4.5 4.0 3.5 3.0 2.5

b1 (OP) b2 (OP) b3 (OP) a1 (TP) a2, a3 (TP)

2.0 1.5 1.0 0.0

(c)

0.1

0.2

0.3

0.4

0.5

Strain

FIG. 3. Variation in 共a兲 the total energy, 共b兲 the stress, and 共c兲 the lattice constants of bcc V under 关100兴 tension as a function of the applied strain. Open symbols refer to the primary tetragonal deformation path, closed symbols to the secondary orthorhombic deformation path. The bifurcation from the PTP to the SOP occurs at a strain of 0.06.

corresponding to a slight volume expansion. Upon further increased tensile strain the total energy reaches a minimum for a special bct structure at ⑀ = 0.494 for V, ⑀ = 0.479 for Nb and at ⑀ = 0.438 for Ta. The ITS and the critical strains for all three metals calculated along the PTP are compiled in Table 0.40

Orthorhombic path Tetragonal path

0.35 0.30 0.25

σ11 (GPa)

bcc

fct

0.25

Lattice parameters (A)

x ~ x

0.30

0.20 0.15 0.10 0.05 0.00

bcc-Nb

-0.05

(a)

0.0

0.1

0.2

0.3

0.4

0.5

Strain

30 25 20 15 10 5 0 -5 -10 -15 -20 -25 -30

(b)

Orthorhombic path Tetragonal path

bcc-Nb 0.0

0.1

0.2 0.3 Strain

0.4

0.5

5.5 bcc-Nb

5.0 Lattice parameters (A)

a 2 = a0

Orthorhombic path Tetragonal path

0.35

σ11 (GPa)

a1 = b1 = a′

bct

∆E = E(ε) - E(0) (eV/atom)

bct

∆E = E(ε) - E(0) (eV/atom)

a2 = 2 a′ 2

4.5 4.0 3.5 3.0 2.5

b1 (OP) b2 (OP) b3 (OP) a1 (TP) a2, a3 (TP)

2.0 1.5 1.0

(c)

0.0

0.1

0.2 0.3 Strain

0.4

0.5

FIG. 4. Variation in 共a兲 the total energy, 共b兲 the stress, and 共c兲 the lattice constants of bcc Nb under 关100兴 tension as a function of the applied strain. Open symbols refer to the primary tetragonal deformation path, closed symbols to the secondary orthorhombic deformation path. The bifurcation from the PTP to the SOP occurs at a strain of 0.05.

094108-5

PHYSICAL REVIEW B 81, 094108 共2010兲

NAGASAKO et al. 0.40

0.25 σ11 (GPa)

∆E = E(ε) - E(0) (eV/atom)

0.30

0.20 0.15 0.10 0.05 0.00

bcc-Ta

-0.05

(a)

30 25 20 15 10 5 0 -5 -10 -15 -20 -25 -30

Orthorhombic path Tetragonal path

0.35

0.0

0.1

0.2 0.3 Strain

0.4

0.5

(b)

Orthorhombic path Tetragonal path

bcc-Ta 0.0

0.1

0.2

0.3

0.4

0.5

Strain

5.5 bcc-Ta

Lattice parameters (A)

5.0 4.5 4.0 3.5 3.0 2.5

b1 (OP) b2 (OP) b3 (OP) a1 (TP) a2, a3 (TP)

2.0 1.5 1.0

(c)

0.0

0.1

0.2

0.3

0.4

0.5

Strain

FIG. 5. Variation in 共a兲 the total energy, 共b兲 the stress, and 共c兲 the lattice constants of bcc Ta under 关100兴 tension as a function of the applied strain. Open symbols refer to the primary tetragonal deformation path, closed symbols to the secondary orthorhombic deformation path. The bifurcation from the PTP to the SOP 共equivalent to a shear instability of the bct lattice兲 occurs at a strain of ⑀ = 0.16, i.e., it is almost coincident with the stress maximum along the PTP.

II. For Nb we note a very good agreement with the results of Luo et al.21 The dimensionless ITSs 쐓 = max / E具100典 ⬃ 0.10– 0.11 reached along the PTP are somewhat larger than those calculated of bcc Mo and W, reflecting a modest asymmetry of the stress-strain curve. If the constraint of a tetragonal guiding symmetry is relaxed, a bifurcation to the SOP occurs at low values of the critical strain, ⑀c = 0.06 and 0.05 for V and Nb, but only at ⑀c = 0.16 for Ta. For Ta this critical strain is almost identical to the critical strain at which the stress maximum is reached along the PTP, while for V and Nb the ITS is limited by the bifurcation to the SOP. Figure 6 shows the variation in the elastic constants of all three metals under uniaxial strain along the 关100兴 direction, referred to a face-centered tetragonal lattice. The important

results are the following: 共i兲 within a fct reference frame the condition c22 = c23 is fulfilled at strains of 0.06, 0.05, and 0.18 for V, Nb, and Ta, respectively. Within a bct reference frame, the condition for a bifurcation is c44 = 0. 共ii兲 At these strains the symmetry will change from tetragonal to orthorhombic under purely uniaxial loading. The behavior of V and Nb at the bifurcation point differs substantially from that of Ta. For V and Nb the energy-strain curves of the PTP and SOP are tangent at the bifurcation point, the difference between the lattice constants b2 and b3 changes continuously, the stress continues to increase after the bifurcation. Hence for V and Nb the branching from the PTP to the SOP is a continuous second order structural transformation from the bct to a face-centered orthorhombic structure induced by purely uniaxial loading which occurs before the ideal tensile strength is reached. For Ta the condition c22 = c23 共within the fct reference frame兲 or c44 = 0 共within a bct description of the deformed structure兲 leads to a shear instability at the stress maximum under uniaxial tension. This means that even under strict uniaxial load, Ta fails not by cleavage but by shear. The unstable saddle-point configuration reached along the SOP is a “special” bct structure which is energetically degenerate with the metastable fct structure reached at large strains on the PTP. In fact, both structures are related through a rigid rotation about the b3 axis, the axial ratio of the fct structure is just 1 / 冑2 times the axial ratio of the bct structure 共a1 / a2 = 1.81兲. At a strain of about 0.41 the energy along the SOP falls to an energy minimum. The configuration corresponding to this minimum is a bcc structure rotated about the b2 axis relative to the original bcc structure. The restoring strain of ⑀ = 0.41 is very close to the value of ⑀ = 冑2 − 1 = 0.414 calculated for a strictly volume-conserving deformation. The bct saddle-point configuration reached on the SOP under uniaxial 具100典 loading is identical to that reached under shear along a 具111典 axis, as will be discussed in more detail below. Hence also along the SOP the bcc metals are predicted to fail not by cleavage, but by shearing. Hence we find that along the PTP the sequence of the stress-free structures is bcc, fcc, bct 关corresponding to scenario 共3兲 discussed by Milstein et al.8,9,11兴 for V, Nb, and Ta, as for the other bcc transition metals 共Mo, W, Fe兲 investigated so far. For Ta the criterion c22 = c23 for a bifurcation to an orthorhombic path is satisfied only for a large strain co-

TABLE II. Ideal tensile strengths max, critical strain ⑀c, Young’s modulus E关100兴 of V, Nb and Ta under uniaxial 关100兴 loading, as determined by the stress maximum along the tetragonal and orthorhombic deformation paths. Orthorhombic

V Nb Ta Mo W

This work This work Ref. 21 This work Ref. 21 Ref. 19

Tetragonal

E具100典

max

⑀c

max / E具100典

max

⑀c

max / E具100典

160 148 165 146 370 407

11.5 12.5 13.1 13.6

0.10 0.11 0.12 0.16

0.07 0.09 0.08 0.09

17.8 17.2 18.8 13.4 28.8 29.5

0.17 0.17 0.18 0.16 0.13 0.13

0.11 0.12 0.11 0.10 0.08 0.07

094108-6

PHYSICAL REVIEW B 81, 094108 共2010兲

ANOMALIES IN THE RESPONSE OF V, Nb, AND Ta TO… 300

300

bcc-V (related to a fct lattice)

200

c11 c12 c22 c23 c44 c55

150 100 50 0 -50 0.00

0.05

0.10

0.15

0.20

0.25

50

0.05

0.10

0.15

0.20

0.25

0.30

Strain 300

bcc-Nb (related to a fct lattice)

bcc-Ta (related to a fct lattice)

250

200

Elastic constant (GPa)

Elastic constant (GPa)

100

(b)

250 c11 c12 c22 c23 c44 c55

150 100 50 0

(c)

c11 c12 c22 c23 c44 c55

150

-50 0.00

0.30

Strain

-50 0.00

200

0

(a) 300

bcc-V (related to a bct lattice)

250 Elastic constant (GPa)

Elastic constant (GPa)

250

200

c11 c12 c22 c23 c44 c55

150 100 50 0

0.05

0.10

0.15 Strain

0.20

0.25

-50 0.00

0.30

(d)

0.05

0.10

0.15 Strain

0.20

0.25

0.30

FIG. 6. 共Color online兲 Variation in the elastic constants c11, c12, c22, c23, c44, and c55 共related to a face-centered tetragonal lattice兲 of 共a兲 V, 共c兲 Nb, and 共d兲 Ta along the primary tetragonal deformation path as a function of uniaxial 关100兴 strain. For V we show also the elastic constants related to a bct reference frame 共b兲, in this case the elastic constants reduce to c11, c12, and c44 in the bcc limit. Note that the condition for the bifurcation to an orthorhombic lattice is c22 = c23 in the fct reference frame 共contraction/expansion along the fct axes—cf. Fig. 2兲, but c44 = 0 in the bct reference frame 共contraction/expansion along the face-diagonals of the bct basis plane兲.

incident with the critical strain for tensile failure along the PTP. Hence the situation is similar to that described before for Mo 共Ref. 21兲 and Fe.32 If the saddle-point structure on the SOP is described within the bct reference frame used for tetragonal deformation under 关100兴 tension, the orthorhombic instability corresponds to a shear instability with c44 = 0. For V and Nb the bifurcation to the SOP occurs already at much smaller strains, the failure mode is determined by the fct saddle-point structure along the SOP. The ITS is reduced from 17.8 GPa to 11.5 GPa for V, and from 17.2 to 12.5 GPa for Nb. The value for Nb is in good agreement with the earlier calculations of Luo it et al.21 For Ta the stress maximum is 13.4 GPa along the tetragonal and 13.6 GPa along the orthorhombic deformation path, i.e the values agree within the computational accuracy. For all three metals the stress-strain curves along the PTP are too asymmetric to be fitted by a sinusoidal curve, leading to a dimensionless ITS of 쐓 ⬃ 0.10– 0.12 which is larger than that calculated for the other bcc transition metals. The stress-strain curve for the SOP is more symmetric, the dimensionless ITS assumes values of 0.07 to 0.09 comparable with those derived for Mo, W, and Fe. V. RESPONSE TO SHEAR DEFORMATIONS ALONG THE Š111‹ DIRECTION

Figure 7 shows the computational cells used for simulating shear deformations along a 具111典 direction on the 兵211其

and 兵110其 planes. The undeformed cells are orthorhombic, with lattice parameters aSC, bSC, and cSC as defined in the figure. The shear deformation was applied uniformly to the supercell 共affine shear loading兲. This means that in principle, the calculations could also have been performed with a primitive cell instead. The supercells have been used for computational convenience. With current optimizer relaxation of all transverse stress components to zero values is easier in the supercell geometry. Because of the threefold rotational symmetry around the 具111典 axis the relaxed shear modulus G具111典 is the same for all common bcc slip systems, 兵110其具111典, 兵211其具111典, and 兵321其具111典 共here we discuss only the former two兲. Earlier work of Morris et al.19–21,61 on the response of W and Mo to shear loading has demonstrated that the relaxed energy/ strain, stress/strain curves, and the ideal shear strengths are very similar for all three slip systems. The changes in symmetry during shear deformation have been discussed in detail by Roundy et al.19 and Krenn et al.,20 using slightly different geometrical arguments. The 兵110其具111典 shear system is symmetric, while the 兵211其具111典 and 兵321其具111典 are not, i.e., slip in the “easy” direction has a lower shear strength than in the “hard” direction. Here we shall restrict our attention to slip in the easy 共weak兲 direction. Upon shearing the bcc lattice parallel to the 共211兲 plane a mirrored bcc lattice is created at a strain of ␥ = 冑2 / 2 ⬃ 0.71 共the “twining” strain兲 if relaxation is excluded. If only a single maximum in the total energy exists for strains from 0 to 0.71, symmetry dictates that it must be

094108-7

PHYSICAL REVIEW B 81, 094108 共2010兲

NAGASAKO et al.

z : [ 1 1 2]

aSC

aSC

bSC

cSC

bSC

cSC β SC α SC γ SC

x : [111]

b

β

c

a

y : [ 1 10]

β SC

Unstrained structure

α SC

c

β

γ SC

a

b

Saddle-point structure

(a) Supercells used for {211} shear

aSC

cSC

z : [1 1 0] b

β SC

α

α SC

cSC

a

β γ

γ SC

x : [111]

aSC

c

bSC

y : [ 1 1 2]

Unstrained structure

b

α SC β SC

c

α β γ

γ SC

a

bSC

Saddle-point structure

(b) Supercells used for {110} shear FIG. 7. 共Color online兲 Supercells used to simulate shear deformations along the 具111典 direction. Part 共a兲 shows the cell used for 兵211其具111典 shear, the left part represents the undeformed cell with bcc symmetry, the right part the bct structure at the saddle-point configuration. The primitive cells inscribed in the supercells are shown in red 共black兲. Part 共b兲 shows the starting 共bcc兲 and saddlepoint 共bct兲 structures for 兵110其具111典 shear. At intermediate strains the symmetry is reduced to monoclinic and triclinic under 兵211其具111典 and 兵110其具111典 shears, respectively. The monoclinic cells inscribed in the supercells which become the bct cells at the saddle-point structure are indicated by the blue 共gray兲 circles.

located at ␥ ⬃ 0.35, and the inflection point must fall around 0.17. Along this deformation path the symmetry changes from cubic to monoclinic and further to orthorhombic at the saddle point 共see Fig. 7兲. For W it has been found that relaxation has only a very small influence on the stress under 共211兲关111兴 strain along the easy direction. This has been attributed to the elastic isotropy of W. Unrelaxed 共110兲关111兴 shear reduces the symmetry from cubic to triclinic, the first energy maximum is found when the deformation path passes through a configuration with monoclinic symmetry. For both Mo and W a significantly stronger relaxation has been reported for 共110兲关111兴—relaxation is necessary to recover the bcc structure at a strain of ␥ ⬃ 0.6. For Mo, Luo et al.21 have reported that due to relaxation, the saddle-point structure under 共110兲关111兴 shear is very similar to the bct saddle point found for the 共211兲关111兴 slip systems. Still, for both Mo and W the stress-strain curves are almost identical for all three slip systems, they have a symmetric sinusoidal shape leading

to a reduced shear strength of max / G具111典 ⬃ 0.11. Luo et al. have also calculated the shear strength of bcc Nb. In this case the stress-strain curves for the 共110兲关111兴 and 共211兲关111兴 shear systems are more distinctly different than for Mo and more asymmetric, leading to a higher value of the reduced shear strength of ⬃0.15– 0.18, although the actual shear strength is much lower. The results for the three V-group metals compiled in Figs. 8–10 show that the response of V and Nb on one side and Ta on the other side are significantly different, although the values of the ideal shear strengths are not. For all three metals the ideal shear strength calculated for both slip systems reaches only half the value found for Mo and W in the neighboring column of the Periodic Table. For V and Nb the stress-strain curves are strongly asymmetric—as we shall show below, this is related to a low value of the shear modulus G具111典, a strong anisotropy of the elastic shear constants 共which is, admittedly, strongly overestimated by the ab initio calculations兲 and strong relaxations under shear loading. For Ta the stress-strain curves are only weakly asymmetric, the reduced shear strength comes close to that calculated for Mo and W. For V, slightly different saddle-point configurations located at strains of 0.28 and 0.32 are found under 兵110其具111典 and 兵211其具111典 shear deformations. These differences are related to different degrees of relaxation changing in both cases significantly as a function of strain. Up to a strain of about 0.08 both shears lead to an increase of the lattice constant bSC, a decrease of cSC, while aSC remains almost constant 关see Figs. 8共c兲 and 8共d兲兴. In this regime only the shearing angle SC increases linearly with strain, while the other angles remain almost unchanged even under 兵110其具111典 shear where the symmetry is reduced to triclinic. Up to this point the deformation occurs at almost constant volume. At a strain of ⑀ = 0.08 the lattice constant cSC reaches a minimum. At larger strains the lattice expands strongly along the bSC and cSC directions and contracts by a comparable amount along aSC—together this results in a volume expansion reaching about 1% at the saddle-point configurations and decreasing again at even larger strains. The volume expansion is coupled to a strong increase in energy. Qualitatively, the relaxation pattern is the same for both shear systems, but the variation in the lattice constants is much larger under 兵211其具111典 shear while the symmetry remains at least monoclinic at all strains. At the saddle points we find that both lattice constants and angles agree with a bct structure, as shown in Fig. 7. In the saddle-point configurations the monoclinic and triclinic lattices of the 兵211其具111典 and 兵110其具111典 shear systems adopt tetragonal symmetry, the lattice constants correspond exactly to those determined along the PTP under uniaxial tension 共which is just rotated with respect to the bct saddle-point structure reached along the SOP兲. The most striking feature, however, is the strongly asymmetric character of the stress-strain curve. Due to the low value of the shear modulus, the stress increases very slowly, the stress-strain curve shows upward curvature. The G具111典 shear modulus derived from the initial slope of the stressstrain curve of V is G具111典 = 31.3⫾ 4 GPa, in reasonable agreement with the value derived from the elastic constants. As discussed above, energy and stress begin to increase at a

094108-8

PHYSICAL REVIEW B 81, 094108 共2010兲

ANOMALIES IN THE RESPONSE OF V, Nb, AND Ta TO… 0.20 ∆E = E(ε) - E(0) (eV/atom)

10

{110} {211}

bcc-V

bcc-V

8 6

0.15 σ31 (GPa)

4

0.10

2 0 -2 -4

0.05

-6 {110} {211}

-8

0.00

-10

0.0

0.1

0.2 0.3 Strain

2.65 2.60 2.55 2.50 2.45 2.40 4.50

0.0

0.1

(b)

0.2 0.3 Strain

0.4

0.5

bcc-V {110}

2.50

4.30

bSC=b

4.20 7.80 7.60 7.40 7.20 7.00

aSC

2.40 8.00 7.80 7.60 7.40 7.20

Lattice parameters (A)

4.40

bSC

4.70 4.50 4.30

cSC

cSC

4.10

90

αSC βSC γSC β

80 70 0.0

0.1

0.2

0.3 Strain

110 100 90 αSC βSC γSC

80 70 60

0.4

0.5

(d)

Angle (degree)

100

0.0

0.1

0.2

0.3 Strain

0.4

2.70 2.60 2.50 2.40 2.30 2.20 4.70

bcc-V {110} a c b

4.50 4.30 4.10

120 Angle (degree)

Angle (degree)

0.5

2.60 aSC=a c

110

(c)

0.4

2.70

bcc-V {211}

Lattice parameters (A)

Lattice parameters (A)

(a)

0.5

(e)

115 110 105 100 95 90 85 80 75

α β γ

0.0

0.1

0.2

0.3

0.4

0.5

Strain

FIG. 8. Variation in 共a兲 the total energy, 共b兲 the stress, 共c兲–共d兲 the lattice constants and angles of the computational super-cell, and 共e兲 of the distorted body-centered cell for bcc V as a function of the applied strain under 兵110其具111典 and 兵211其具111典 shear deformations.

strain large enough such that a pure shear deformation is insufficient to relax all lateral stresses and an expansion of the volume takes place. For both shear systems, the stress maximum is reached at a failure strain of about 0.2—this value is much larger than half of the strain at which the saddle point is located. The ideal tensile strength is 6.5 GPa for shearing along the 兵110其 and 5.5 GPa along the 兵211其 planes, the reduced shear strengths are 0.20 and 0.17, respectively 共see Table III兲. This means that the reduced shear strength is much higher than for Mo and W, although the actual shear strength reaches not even half this value. Nb shows a behavior under shear which is very similar to that discussed above for V. From the initial slope of the stress-strain curve we calculate a shear modulus of G具111典 ⬃ 22⫾ 4 GPa, in good agreement with the elastic constants. A remarkable difference is that the initial contraction of the lattice constant cSC at smaller strains has almost disappeared, and that aSC begins to shrink already at smaller strains. But again we observe a distinct change in the relaxation mode at a strain of ␥ ⬃ 0.08, slightly below the inflection point on the stress-strain curve. At larger strains, relaxation leads to a substantial volume expansion reaching 2% at the saddlepoint configuration. The saddle-point structures assumed at ␥ ⬃ 0.33 共for 兵211其具111典 shear兲 and ␥ ⬃ 0.29 共for 兵110其具111典 shear兲 are bct and agree with those assumed on the SOP under uniaxial 关100兴 tension 共cf. Figs. 9 and 4兲. The maximum shear stress is 6.0 GPa 共at a failure strain of ␥c = 0.2兲 for shearing parallel to the 兵211其 plane, and 7.8 GPa 共at ␥c

= 0.2兲 for shearing along 兵110其. These values are in good agreement with those of Luo et al.,21 although we find a slightly larger difference between both shear systems. The reduced value of the ideal shear strength is even larger than for V. For Ta the initial slope of the stress-strain curve yields G具111典 ⬃ 58⫾ 1 GPa in excellent agreement with the elastic constants. Only very modest relaxations are observed up to strains of about 0.1. Beyond this point, the lattice constant cSC increases strongly with increasing strain, while bSC and aSC undergo only a more modest expansion and contraction, respectively. These relaxations are also associated with an increasing volume expansion reaching 2% at the saddle point. The saddle-point configurations are reached at ␥ = 0.29 共for 兵110其具111典 shear兲 and ␥ = 0.32 共for 兵211其具111典 shear兲. The bct lattice constants of the saddle-point structures are a = c = 2.795 Å and b = 4.769 Å 共for 兵211其具111典 shear, those for 共110兲关111兴 shear agree within 0.01 Å兲, to be compared with a = 4.781 Å, b = c = 2.792 Å calculated along the PTP under uniaxial tension. The values of the ideal shear strength are 7.1 共6.5兲 GPa, at critical strains of ␥c = 0.22共0.20兲 for shearing parallel to the 兵110其 共兵211其 planes兲, respectively 共see Table III兲. Although they are much lower than those for Mo and W, all three metals show the same reduced shear strength. Hence for Ta the low value of the ideal shear strength is exactly as expected from the soft elastic shear modulus, while for V and Nb the extremely low shear modulus is not reflected by a similarly low value of the ideal shear strength.

094108-9

PHYSICAL REVIEW B 81, 094108 共2010兲

NAGASAKO et al. 0.20

10 8

0.15 σ31 (GPa)

4

0.10

-6

{110} {211} 0.0

0.1

0.2

bcc-Nb {211} aSC=a c

Lattice parameters (A)

0.4

0.5

0.0

bSC=b

cSC

0.1

(b)

2.90 2.85 2.80 2.75 2.70 8.80 8.60 8.40 8.20 8.00

0.2 0.3 Strain

Angle (degree)

90

αSC βSC γSC β

80 70 0.0

0.1

0.2

0.3 Strain

bSC

5.40 5.20 5.00 4.80 4.60

cSC

110 100 90 αSC βSC γSC

80 70 60

0.4

0.5

(d)

0.5

aSC

120

100

0.4

bcc-Nb {110}

Angle (degree)

Lattice parameters (A) Angle (degree)

0.3

{110} {211}

-8 -10

Strain

110

(c)

0 -2 -4

(a)

9.00 8.80 8.60 8.40 8.20 8.00

2

0.05

0.00

2.90 2.85 2.80 2.75 2.70 5.00 4.90 4.80 4.70 4.60

bcc-Nb

6

Lattice parameters (A)

∆E = E(ε) - E(0) (eV/atom)

bcc-Nb

0.0

0.1

0.2

0.3 Strain

0.4

0.5

(e)

2.90 2.85 2.80 2.75 2.70 5.00 4.90 4.80 4.70 4.60

bcc-Nb {110} a c b

115 110 105 100 95 90 85 80 75

α β γ

0.0

0.1

0.2

0.3

0.4

0.5

Strain

FIG. 9. Variation in 共a兲 the total energy, 共b兲 the stress, 共c兲–共d兲 the lattice constants and angles of the computational super-cell and 共e兲 of the distorted body-centered cell for Nb as a function of the applied strain under 兵110其具111典 and 兵211其具111典 shear deformations. VI. DISCUSSION AND CONCLUSIONS

We have demonstrated using ab initio DFT calculations that the response of body-centered cubic V and Nb to tensile and shear loading differs substantially from that of other bcc transition metals such as Mo, W, and Fe, but also from that of the heaviest metal of the V group, Ta. For these metals the stress-strain curves under tension or shear display a symmetric sinusoidal shape, with a period determined by the nearest extremum on the deformation path. Under uniaxial 具100典 tension this is a maximum corresponding to a fcc structure adopted under volume conservation at the Bain strain of ⑀ = 冑3 2 − 1 ⬃ 0.26. For all types of shear along the 具111典 this is a bct structure formed under volume conservation at a shear strain of ␥ = 冑2 / 4 ⬃ 0.35, i.e., at half the “twinning” strain recovering the bcc structure. As the initial slope of the stressstrain curve is determined by the relaxed tensile and shear modulus, respectively, the ideal tensile and shear strengths obey the relations

max =

0.26 E具100典 = 0.08E具100典 ,

共3兲

max =

0.35 G具111典 = 0.11G具111典 .

共4兲

For Mo and W the calculated moduli and ideal strength obey these relations with good accuracy. For V and Nb we

find that under uniaxial 具100典 loading a bifurcation from the primary tetragonal to a secondary orthorhombic deformation path occurs before reaching the stress maximum, strongly limiting the ideal tensile strength. Due to a shear instability, an orthorhombic deformation can occur under purely uniaxial load. It is interesting to correlate this shear instability induced by uniaxial strain to the softening of c44 under homogeneous compression. It has been shown that for V c44 vanishes at a pressure of about 60 GPa, leading to bcc → rhombohedral structural transition21,41,42,44 and that this phase transition is associated with the nesting properties of the Fermi surface and an electronic topological transition. While the homogeneous compression of the bcc lattice merely changes the nesting vector, a uniaxial strain changes the symmetry and therefore the topology of the Fermi surface. The saddle-point structure along the SOP is a special bct structure which can be made to coincide with the fct local energy minimum along the PTP by a rigid rotation and which is also identical to the saddle-point structure under shear deformation. For Ta the bifurcation to the SOP coincides with the stress-maximum along the PTP 共as has also been found for Mo兲. Because the ideal tensile strength is reached at a shear-unstable configuration, Ta fails under uniaxial loading not by cleavage, but by shear. The stress/tensile-strain curves of all three metals are strongly asymmetric along the PTP, but less so along the SOP. This means that the reduced tensile shear strength 쐓 = max / E具100典 is about 0.07 to 0.09, only

094108-10

PHYSICAL REVIEW B 81, 094108 共2010兲

ANOMALIES IN THE RESPONSE OF V, Nb, AND Ta TO… 0.20

10 8

0.15 σ31 (GPa)

4

0.10

-6

{110} {211} 0.0

0.1

0.2

bcc-Ta {211} aSC=a c

Lattice parameters (A)

0.4

0.5

0.0

bSC=b

cSC

0.1

(b)

2.90 2.85 2.80 2.75 2.70 8.80 8.60 8.40 8.20 8.00

0.2 0.3 Strain

0.4

aSC 2.90

bSC

5.40 5.20 5.00 4.80 4.60

cSC

Angle (degree)

90

αSC βSC γSC β

80 70 0.0

0.1

0.2

0.3

110 100 90 αSC βSC γSC

80 70 60

0.4

0.5

Strain

(d)

0.0

0.1

0.2

0.3

0.4

bcc-Ta {110}

2.85 2.80 2.75 4.90

a c b

4.80 4.70 4.60

120

100

0.5

bcc-Ta {110}

Angle (degree)

Lattice parameters (A) Angle (degree)

0.3

{110} {211}

-8 -10

Strain

110

(c)

0 -2 -4

(a)

9.00 8.80 8.60 8.40 8.20 8.00

2

0.05

0.00

2.90 2.85 2.80 2.75 2.70 5.00 4.90 4.80 4.70 4.60

bcc-Ta

6

Lattice parameters (A)

∆E = E(ε) - E(0) (eV/atom)

bcc-Ta

0.5

Strain

(e)

115 110 105 100 95 90 85 80 75

α β γ

0.0

0.1

0.2

0.3

0.4

0.5

Strain

FIG. 10. Variation in 共a兲 the total energy, 共b兲 the stress, 共c兲–共d兲 the lattice constants and angles of the computational super-cell, and 共e兲 of the distorted body-centered cell for Ta as a function of the applied strain under 兵110其具111典 and 兵211其具111典 shear deformations.

slightly larger than for Mo and W, although the ITS is determined by a different saddle-point configuration. Ta is a special case where the bifurcation point coincides with the inflection point on the PTP energy-strain curve. Hence the tetragonal stress maximum is reached at a shear-unstable configuration. Shearing bcc V or Nb in the 具111典 direction parallel to a 兵110其 or 兵211其 planes leads to strongly asymmetric stressstrain curves. A volume conserving unrelaxed 兵211其具111典 shear recovers the bcc structure at a strain of ␥ = 冑2 / 2, hence by symmetry the saddle-point configuration should fall at ␥ ⬃ 0.35 and the inflection point or stress maximum at ␥c

⬃ 0.175. However, due to a very low relaxed shear modulus G关111兴, the initial slope of the stress-strain curve is very low. The stress begins to increase strongly at ␥ ⬃ 0.08 were the relaxation pattern changes qualitatively, accompanied by an incipient volume expansion. The saddle-point structure for both glide systems has bct symmetry, it is reached at strains between 0.28 and 0.32 depending on the glide plane. For 兵110其具111典 shear a strong relaxation is required to reach this configuration. This bct saddle-point structure is the same as that reached on the SOP under uniaxial 具100典 tension. For V the failure strain is ␥c = 0.20, the ideal shear strength is 6.5 and 5.5 GPa for the 兵110其 and 兵211其 glide planes, respec-

TABLE III. Ideal shear strengths max, critical strain ␥c, shear modulus G关111兴 of V, Nb, and Ta under uniaxial 关100兴 loading, as determined by the stress maximum along the tetragonal and orthorhombic deformation paths. 兵110其具111典

V Nb Ta Mo W

This work This work Ref. 21 This work Ref. 21 Ref. 19

兵211其具111典

G具111典

max

␥c

max / G具111典

max

␥c

max / G具111典

33 31

6.54 7.8 7.6 7.1 16.1 18.2

0.21 0.20 0.22 0.22 0.17 0.17

0.20 0.25

5.5 6.0 6.4 6.5 15.8 18.1

0.21 0.20 0.20 0.201 0.17 0.17

0.17 0.19

53 134 163

094108-11

0.13 0.12 0.11

0.12 0.12 0.11

PHYSICAL REVIEW B 81, 094108 共2010兲

NAGASAKO et al.

tively. The reduced shear strengths are 쐓 = 0.20 and 0.17— i.e., nearly twice as high as expected for a symmetric stressstrain curve and as calculated for Mo and W. Nb follows the same pattern, with an even slightly larger reduced shear strength. In summary: 共i兲 For both V and Nb the ideal tensile strength under 具111典 loading is limited by a bifurcation to an orthorhombic deformation path, but it is still about twice as large as the ideal shear strength for shearing in the 具111典. 共ii兲 The stress-strain curves for V and Nb under shear deformation are strongly asymmetric, the ideal shear strength is much higher than expected on the basis of a very low shear modulus. This reflects an increasing stiffness of the lattice under increasing shear strain, as shown by the relaxation behavior. 共iii兲 The saddle-point configurations reached under tensile and shear loading have the same special bct structure. For this reason and because the ideal shear strength is much lower than the tensile strength, both metals will fail by shear and not by cleavage. 共iv兲 The response of Ta to tensile and shear loading is more similar to that of Mo or W. However, because the stress maximum under tension is reached at a shear-unstable configuration, Ta will also fail by shear and not by cleavage.

*[email protected] †[email protected]

ACKNOWLEDGMENTS

Work at the University of Vienna has been supported by the VASP project and within the University Research Focus “Material Science” and “Computational Science.” We thank T. Bučko for provision of GADGET structural optimization package.

Philos. Mag. A 81, 1725 共2001兲. R. Krenn, D. Roundy, J. W. Morris, Jr., and M. L. Cohen, Mater. Sci. Eng., A 319-321, 111 共2001兲. 21 W. Luo, D. Roundy, M. L. Cohen, and J. W. Morris, Jr., Phys. Rev. B 66, 094110 共2002兲. 22 M. Jahnátek, M. Krajčí, and J. Hafner, Philos. Mag. 87, 1769 共2007兲. 23 M. Jahnátek, M. Krajčí, and J. Hafner, Phys. Rev. B 76, 014110 共2007兲. 24 M. Jahnátek, J. Hafner, and M. Krajčí, Phys. Rev. B 79, 224103 共2009兲. 25 J. Pokluda, M. Černy, P. Šandera, and M. Šob, J. Comput.-Aided Mater. Des. 11, 1 共2004兲. 26 D. M. Clatterbuck, C. R. Krenn, M. L. Cohen, and J. W. Morris, Jr., Phys. Rev. Lett. 91, 135501 共2003兲. 27 H. Kitagawa and S. Ogata, Key Eng. Mater. 161-163, 443 共1999兲. 28 S. Ogata and S. Yip, Science 298, 807 共2002兲. 29 S. Ogata, J. Li, and S. Yip, Phys. Rev. B 71, 224102 共2005兲. 30 M. Černy, M. Šob, J. Pokluda, and P. J. Šandera, J. Phys.: Condens. Matter 16, 1045 共2004兲. 31 M. Šob, L. G. Wang, and V. Vitek, Kovove Mater. 36, 145 共1998兲. 32 D. M. Clatterbuck, D. C. Chrzan, and J. W. Morris, Jr., Acta Mater. 51, 2271 共2003兲. 33 M. Friák, M. Šob, and V. Vitek, Philos. Mag. A 83, 3529 共2003兲. 34 M. Jahnátek, M. Krajčí, and J. Hafner, 共unpublished兲. 35 W. Luo, M. L. Cohen, and J. W. Morris, Jr., Philos. Mag. Lett. 89, 23 共2009兲. 36 J. Trivisonno, S. Vatanayon, M. Wilt, J. Washick, and R. Reifenberger, J. Low Temp. Phys. 12, 153 共1973兲. 37 K. W. Katahara, M. H. Manghnani, and E. Fisher, J. Phys. F: Met. Phys. 9, 773 共1979兲. 20 C.

‡[email protected] §

For Ta the ideal shear strength found in our calculations 关max = 7.1共6.5兲 GPa for 兵110其具111典 and 兵211其具111典 shear兴 is in excellent agreement with experimental estimates based on nanoindentation measurements4 yielding an ideal shear strength of about 7.5 GPa. From the nanoindentation experiments and experimental observations of plastic flow response to large strain impact testing62 it was also suggested the 兵110其具111典 slip system is preferred over the 兵211其具111典 slip system, but we find only very small differences in the limiting shear strengths and in the critical strains. However, it is certainly encouraging to see that experimental and theoretical determinations of the ideal strength of metals begin to converge.

[email protected] 1 A. Kelly and N. H. MacMillan, Strong Solids, 3rd ed. 共Clarendon Press, Oxford, 1986兲. 2 N. Gane and F. P. Bowden, J. Appl. Phys. 39, 1432 共1968兲. 3 S. G. Corcoran, R. J. Colton, E. T. Lilleodden, and W. W. Gerberich, Phys. Rev. B 55, R16057 共1997兲. 4 M. M. Biener, J. Biener, A. M. Hodge, and A. V. Hamza, Phys. Rev. B 76, 165422 共2007兲. 5 C. A. Schuh, J. K. Mason, and A. C. Lund, Nature Mater. 4, 617 共2005兲. 6 C. A. Schuh, Mater. Today 9, 32 共2006兲. 7 J. Frenkel, Z. Phys. 37, 572 共1926兲. 8 R. Hill and F. Milstein, Phys. Rev. B 15, 3087 共1977兲. 9 F. Milstein and K. Huang, Phys. Rev. B 18, 2529 共1978兲. 10 F. Milstein and B. Farber, Phys. Rev. Lett. 44, 277 共1980兲. 11 F. Milstein, J. Marschall, and H. E. Fang, Phys. Rev. Lett. 74, 2977 共1995兲. 12 F. Milstein and S. Chantasiriwan, Phys. Rev. B 58, 6006 共1998兲. 13 A. T. Paxton, P. Gumbsch, and M. Methfessel, Philos. Mag. Lett. 63, 267 共1991兲. 14 W. Xu and J. A. Moriarty, Phys. Rev. B 54, 6941 共1996兲. 15 P. Alippi, P. M. Marcus, and M. Scheffler, Phys. Rev. Lett. 78, 3892 共1997兲. 16 M. Šob, L. G. Wang, and V. Vitek, Mater. Sci. Eng., A 234-236, 1075 共1997兲. 17 M. Šob, L. G. Wang, and V. Vitek, Philos. Mag. B 78, 653 共1998兲. 18 D. Roundy, C. R. Krenn, M. L. Cohen, and J. W. Morris, Jr., Phys. Rev. Lett. 82, 2713 共1999兲. 19 D. Roundy, C. R. Krenn, M. L. Cohen, and J. W. Morris, Jr.,

094108-12

PHYSICAL REVIEW B 81, 094108 共2010兲

ANOMALIES IN THE RESPONSE OF V, Nb, AND Ta TO… 38

H. Kojima, M. Shino, and T. Suzuki, Acta Metall. 35, 891 共1987兲. 39 F. H. Featherston and J. R. Neighbours, Phys. Rev. 130, 1324 共1963兲. 40 K. W. Katahara, M. H. Manghnani, and E. Fisher, J. Appl. Phys. 47, 434 共1976兲. 41 A. Landa, J. Klepeis, P. Söderlind, I. Naumov, O. Velikokhatnyi, L. Vitos, and A. Ruban, J. Phys.: Condens. Matter 18, 5079 共2006兲. 42 L. Koči, Y. Ma, A. R. Oganov, P. Souvatzis, and R. Ahuja, Phys. Rev. B 77, 214101 共2008兲. 43 P. Söderlind, O. Eriksson, J. M. Wills, and A. M. Boring, Phys. Rev. B 48, 5844 共1993兲. 44 Y. Ding, R. Ahuja, J. Shu, P. Chow, W. Luo, and H. K. Mao, Phys. Rev. Lett. 98, 085502 共2007兲. 45 T. Kenichi and A. K. Singh, Phys. Rev. B 73, 224119 共2006兲. 46 Y. Nakagawa and A. D. B. Woods, Phys. Rev. Lett. 11, 271 共1963兲. 47 R. Colella and B. W. Batterman, Phys. Rev. B 1, 3913 共1970兲. 48 W. Luo, R. Ahuja, Y. Ding, and H. Mao, Proc. Natl. Acad. Sci. U.S.A. 104, 16428 共2007兲. 49 C. M. Varma and W. Weber, Phys. Rev. B 19, 6142 共1979兲.

G. Kresse and J. Furthmüller, Comput. Mater. Sci. 6, 15 共1996兲. Kresse and J. Furthmüller, Phys. Rev. B 54, 11169 共1996兲. 52 J. P. Perdew, J. A. Chevary, S. H. Vosko, K. A. Jackson, M. R. Pederson, D. J. Singh, and C. Fiolhais, Phys. Rev. B 46, 6671 共1992兲. 53 P. E. Blöchl, Phys. Rev. B 50, 17953 共1994兲. 54 G. Kresse and D. Joubert, Phys. Rev. B 59, 1758 共1999兲. 55 T. Bučko, J. Hafner, and J. G. Ángyán, J. Chem. Phys. 122, 124508 共2005兲. 56 R. P. Feynman, Phys. Rev. 56, 340 共1939兲. 57 O. H. Nielsen and R. M. Martin, Phys. Rev. Lett. 50, 697 共1983兲. 58 H. J. Monkhorst and J. D. Pack, Phys. Rev. B 13, 5188 共1976兲. 59 M. Methfessel and A. T. Paxton, Phys. Rev. B 40, 3616 共1989兲. 60 P. E. Blöchl, O. Jepsen, and O. K. Andersen, Phys. Rev. B 49, 16223 共1994兲. 61 J. W. Morris, Jr., C. R. Krenn, D. Roundy, and M. L. Cohen, in Phase Transformations and Evolution in Materials, edited by P. E. Turchi and A. Gonis 共TMS, Warrendale, PA, 2000兲, p. 187. 62 P. J. Maudlin, J. F. Bingert, and G. T. Gray, Int. J. Plast. 19, 483 共2003兲. 50

51 G.

094108-13